#------------------------------------------------------------------------------
#$Date: 2016-02-05 00:37:45 +0200 (Fri, 05 Feb 2016) $
#$Revision: 175973 $
#$URL: svn://www.crystallography.net/cod/cif/7/22/32/7223243.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7223243
loop_
_publ_author_name
'Xiao, Bin'
'Schlenz, Hartmut'
'Bosbach, Dirk'
'Suleimanov, Evgeny V.'
'Alekseev, Evgeny V.'
_publ_section_title
;
 The structural effects of alkaline- and rare-earth element incorporation
 into thorium molybdates
;
_journal_issue                   1
_journal_name_full               CrystEngComm
_journal_page_first              113
_journal_paper_doi               10.1039/C5CE02040A
_journal_volume                  18
_journal_year                    2016
_chemical_formula_moiety         K2SrTh2Mo6O24
_chemical_formula_sum            'K2 Mo6 O24 Sr Th2'
_chemical_formula_weight         1589.52
_chemical_name_systematic        K2SrTh2(MoO4)6
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2015-10-12 deposited with the CCDC.
2015-11-12 downloaded from the CCDC.
;
_cell_angle_alpha                101.550(15)
_cell_angle_beta                 102.893(12)
_cell_angle_gamma                97.388(13)
_cell_formula_units_Z            2
_cell_length_a                   8.0197(10)
_cell_length_b                   8.4470(17)
_cell_length_c                   16.030(2)
_cell_measurement_reflns_used    1015
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      30.5850
_cell_measurement_theta_min      3.2464
_cell_volume                     1019.9(3)
_computing_cell_refinement
;
 ?
;
_computing_data_collection
;
 ?
;
_computing_data_reduction
;
 ?
;
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 15.9834
_diffrn_measured_fraction_theta_full 0.979
_diffrn_measured_fraction_theta_max 0.979
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Eos'
_diffrn_measurement_method       '\Mo scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0455
_diffrn_reflns_av_sigmaI/netI    0.1132
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            4424
_diffrn_reflns_theta_full        26.37
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         3.25
_exptl_absorpt_coefficient_mu    21.315
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.12627
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
 ?
;
_exptl_crystal_colour
;
 ?
;
_exptl_crystal_density_diffrn    5.176
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description
;
 ?
;
_exptl_crystal_F_000             1404
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.09
_exptl_crystal_size_min          0.09
_refine_diff_density_max         4.429
_refine_diff_density_min         -5.567
_refine_diff_density_rms         0.848
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.027
_refine_ls_matrix_type           full
_refine_ls_number_parameters     316
_refine_ls_number_reflns         3789
_refine_ls_number_restraints     144
_refine_ls_restrained_S_all      1.006
_refine_ls_R_factor_all          0.0893
_refine_ls_R_factor_gt           0.0526
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_wR_factor_gt          0.1129
_refine_ls_wR_factor_ref         0.1300
_reflns_number_gt                2656
_reflns_number_total             4189
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c5ce02040a2.cif
_cod_data_source_block           K2SrTh2Mo6O24
_cod_depositor_comments
'Adding full bibliography for 7223242--7223245.cif.'
_cod_database_code               7223243
_refine_ls_moeighting_scheme     calc
_refine_ls_moeighting_details
'calc Mo=1/[σ²(Fo²)+(0.0591P)²+0.0000P] Mohere P=(Fo²+2Fc²)/3'
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Th1 Th 0.30732(14) 0.30430(14) 0.50391(7) 0.0109(3) Uani 1 1 d .
Th2 Th 0.07471(14) 0.00516(14) 0.16407(7) 0.0096(3) Uani 1 1 d .
Mo1 Mo 0.52995(15) 0.00066(15) 0.34343(8) 0.0083(3) Uani 1 1 d .
Mo2 Mo -0.08758(15) -0.05415(15) 0.34733(8) 0.0084(3) Uani 1 1 d .
Mo3 Mo -0.14091(15) 0.32176(15) 0.33570(8) 0.0091(3) Uani 1 1 d .
Mo4 Mo 0.46295(15) 0.37230(15) 0.31897(8) 0.0092(3) Uani 1 1 d .
Mo5 Mo 0.61571(16) -0.16765(15) -0.01054(8) 0.0108(3) Uani 1 1 d .
Mo6 Mo 0.22226(15) -0.23380(16) -0.00449(8) 0.0111(3) Uani 1 1 d .
O1 O -0.280(3) 0.442(3) 0.4022(13) 0.013(5) Uani 1 1 d U
O2 O 0.595(3) 0.212(3) 0.2722(14) 0.015(5) Uani 1 1 d U
O3 O 0.658(3) -0.104(2) 0.2699(13) 0.011(4) Uani 1 1 d U
O4 O -0.085(2) 0.130(2) 0.2718(12) 0.007(4) Uani 1 1 d U
O5 O 0.515(3) -0.133(2) 0.4139(13) 0.012(5) Uani 1 1 d U
O6 O -0.027(3) -0.173(2) 0.2574(13) 0.010(4) Uani 1 1 d U
O7 O 0.129(2) -0.255(2) 0.0872(12) 0.004(4) Uani 1 1 d U
O8 O 0.407(2) 0.495(2) 0.4187(13) 0.009(4) Uani 1 1 d U
O9 O 0.119(2) 0.056(2) 0.4150(12) 0.008(4) Uani 1 1 d U
O10 O 0.044(3) -0.178(2) -0.0778(12) 0.008(4) Uani 1 1 d U
O11 O 0.487(3) 0.529(3) 0.2638(14) 0.015(5) Uani 1 1 d U
O12 O -0.206(2) 0.122(2) 0.4029(13) 0.007(4) Uani 1 1 d U
O13 O 0.465(2) 0.196(2) 0.4059(12) 0.004(4) Uani 1 1 d U
O14 O 0.388(3) -0.113(3) -0.0635(13) 0.015(5) Uani 1 1 d U
O15 O -0.139(3) -0.209(3) 0.4032(13) 0.013(5) Uani 1 1 d U
O16 O 0.792(3) -0.145(3) 0.0847(15) 0.022(5) Uani 1 1 d U
O17 O 0.195(3) -0.437(2) -0.0581(13) 0.011(4) Uani 1 1 d U
O18 O -0.102(3) 0.449(3) 0.2657(15) 0.020(5) Uani 1 1 d U
O19 O 0.252(3) 0.261(3) 0.2552(14) 0.014(5) Uani 1 1 d U
O20 O 0.467(3) -0.213(3) 0.0675(14) 0.020(5) Uani 1 1 d U
O21 O 0.336(2) -0.055(2) 0.2598(12) 0.007(4) Uani 1 1 d U
O22 O 0.599(3) -0.371(3) -0.0755(15) 0.024(6) Uani 1 1 d U
O23 O 0.722(2) -0.037(2) -0.0736(12) 0.008(4) Uani 1 1 d U
O24 O 0.057(3) 0.375(3) 0.4256(15) 0.022(5) Uani 1 1 d U
Sr1 Sr -0.3335(7) -0.3842(7) 0.1608(4) 0.0652(15) Uani 1 1 d .
K1 K 0.1924(10) -0.2872(10) 0.4337(5) 0.0270(18) Uani 1 1 d .
K2 K -0.1465(11) -0.5025(10) -0.1598(6) 0.032(2) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sr Sr -1.5307 3.2498 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Th Th -7.2400 8.8979 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O24 Th1 O13 109.7(7) . .
O24 Th1 O9 72.0(7) . .
O13 Th1 O9 76.0(6) . .
O24 Th1 O15 88.3(8) . 2_556
O13 Th1 O15 138.2(7) . 2_556
O9 Th1 O15 74.4(7) . 2_556
O24 Th1 O1 76.0(7) . 2_566
O13 Th1 O1 142.7(7) . 2_566
O9 Th1 O1 137.3(7) . 2_566
O15 Th1 O1 77.2(7) 2_556 2_566
O24 Th1 O8 73.9(7) . .
O13 Th1 O8 65.2(6) . .
O9 Th1 O8 114.1(6) . .
O15 Th1 O8 155.6(7) 2_556 .
O1 Th1 O8 82.3(7) 2_566 .
O24 Th1 O5 156.8(7) . 2_656
O13 Th1 O5 76.5(7) . 2_656
O9 Th1 O5 88.6(6) . 2_656
O15 Th1 O5 74.0(7) 2_556 2_656
O1 Th1 O5 113.2(7) 2_566 2_656
O8 Th1 O5 127.1(7) . 2_656
O24 Th1 O8 124.7(7) . 2_666
O13 Th1 O8 84.2(6) . 2_666
O9 Th1 O8 158.1(6) . 2_666
O15 Th1 O8 116.7(6) 2_556 2_666
O1 Th1 O8 64.6(7) 2_566 2_666
O8 Th1 O8 64.2(7) . 2_666
O5 Th1 O8 77.5(6) 2_656 2_666
O24 Th1 Mo4 111.1(5) . 2_666
O13 Th1 Mo4 116.3(4) . 2_666
O9 Th1 Mo4 163.5(5) . 2_666
O15 Th1 Mo4 89.4(5) 2_556 2_666
O1 Th1 Mo4 36.9(5) 2_566 2_666
O8 Th1 Mo4 81.9(4) . 2_666
O5 Th1 Mo4 84.0(4) 2_656 2_666
O8 Th1 Mo4 32.1(4) 2_666 2_666
O24 Th1 Mo4 82.2(6) . .
O13 Th1 Mo4 37.5(5) . .
O9 Th1 Mo4 90.6(5) . .
O15 Th1 Mo4 164.2(5) 2_556 .
O1 Th1 Mo4 112.4(5) 2_566 .
O8 Th1 Mo4 30.0(4) . .
O5 Th1 Mo4 111.3(5) 2_656 .
O8 Th1 Mo4 79.0(5) 2_666 .
Mo4 Th1 Mo4 105.79(4) 2_666 .
O24 Th1 K1 154.8(6) . 2_656
O13 Th1 K1 54.3(4) . 2_656
O9 Th1 K1 116.0(5) . 2_656
O15 Th1 K1 116.6(5) 2_556 2_656
O1 Th1 K1 105.0(5) 2_566 2_656
O8 Th1 K1 81.2(5) . 2_656
O5 Th1 K1 46.3(5) 2_656 2_656
O8 Th1 K1 42.6(5) 2_666 2_656
Mo4 Th1 K1 68.49(12) 2_666 2_656
Mo4 Th1 K1 74.12(13) . 2_656
O24 Th1 K1 45.5(6) . 1_565
O13 Th1 K1 104.6(5) . 1_565
O9 Th1 K1 114.5(5) . 1_565
O15 Th1 K1 114.3(5) 2_556 1_565
O1 Th1 K1 52.1(5) 2_566 1_565
O8 Th1 K1 41.4(5) . 1_565
O5 Th1 K1 156.6(5) 2_656 1_565
O8 Th1 K1 79.4(5) 2_666 1_565
Mo4 Th1 K1 74.43(12) 2_666 1_565
Mo4 Th1 K1 67.10(12) . 1_565
K1 Th1 K1 114.92(13) 2_656 1_565
O10 Th2 O16 75.8(7) 2 1_455
O10 Th2 O19 82.8(7) 2 .
O16 Th2 O19 148.0(8) 1_455 .
O10 Th2 O23 77.1(7) 2 2_655
O16 Th2 O23 114.6(7) 1_455 2_655
O19 Th2 O23 82.7(7) . 2_655
O10 Th2 O7 117.6(6) 2 .
O16 Th2 O7 75.7(7) 1_455 .
O19 Th2 O7 136.0(7) . .
O23 Th2 O7 66.6(6) 2_655 .
O10 Th2 O21 147.6(6) 2 .
O16 Th2 O21 135.7(7) 1_455 .
O19 Th2 O21 71.1(7) . .
O23 Th2 O21 80.7(6) 2_655 .
O7 Th2 O21 73.3(6) . .
O10 Th2 O6 137.0(7) 2 .
O16 Th2 O6 72.4(7) 1_455 .
O19 Th2 O6 110.7(7) . .
O23 Th2 O6 143.1(7) 2_655 .
O7 Th2 O6 81.6(6) . .
O21 Th2 O6 72.3(6) . .
O10 Th2 O4 85.2(7) 2 .
O16 Th2 O4 83.4(7) 1_455 .
O19 Th2 O4 71.2(7) . .
O23 Th2 O4 150.0(6) 2_655 .
O7 Th2 O4 143.3(6) . .
O21 Th2 O4 103.5(6) . .
O6 Th2 O4 63.2(6) . .
O10 Th2 Mo6 95.4(5) 2 .
O16 Th2 Mo6 85.3(6) 1_455 .
O19 Th2 Mo6 120.5(5) . .
O23 Th2 Mo6 40.2(4) 2_655 .
O7 Th2 Mo6 28.3(4) . .
O21 Th2 Mo6 82.2(4) . .
O6 Th2 Mo6 109.9(5) . .
O4 Th2 Mo6 168.3(4) . .
O10 Th2 Mo2 119.7(5) 2 .
O16 Th2 Mo2 81.7(6) 1_455 .
O19 Th2 Mo2 88.8(5) . .
O23 Th2 Mo2 160.1(4) 2_655 .
O7 Th2 Mo2 109.4(4) . .
O21 Th2 Mo2 79.6(5) . .
O6 Th2 Mo2 27.9(5) . .
O4 Th2 Mo2 36.7(4) . .
Mo6 Th2 Mo2 137.72(5) . .
O10 Th2 K2 40.8(5) 2 2
O16 Th2 K2 113.9(6) 1_455 2
O19 Th2 K2 42.0(5) . 2
O23 Th2 K2 74.5(5) 2_655 2
O7 Th2 K2 140.0(5) . 2
O21 Th2 K2 110.2(4) . 2
O6 Th2 K2 138.2(5) . 2
O4 Th2 K2 76.2(5) . 2
Mo6 Th2 K2 111.69(14) . 2
Mo2 Th2 K2 110.36(14) . 2
O10 Th2 Sr1 109.2(5) 2 .
O16 Th2 Sr1 35.7(6) 1_455 .
O19 Th2 Sr1 142.3(5) . .
O23 Th2 Sr1 134.3(4) 2_655 .
O7 Th2 Sr1 71.1(4) . .
O21 Th2 Sr1 103.3(4) . .
O6 Th2 Sr1 37.3(4) . .
O4 Th2 Sr1 74.3(4) . .
Mo6 Th2 Sr1 94.50(8) . .
Mo2 Th2 Sr1 53.93(8) . .
K2 Th2 Sr1 139.52(14) 2 .
O21 Mo1 O5 106.6(9) . .
O21 Mo1 O3 92.8(9) . .
O5 Mo1 O3 101.6(9) . .
O21 Mo1 O13 94.8(8) . .
O5 Mo1 O13 102.0(9) . .
O3 Mo1 O13 152.0(8) . .
O21 Mo1 O12 154.5(8) . 1_655
O5 Mo1 O12 98.1(8) . 1_655
O3 Mo1 O12 75.7(8) . 1_655
O13 Mo1 O12 86.1(7) . 1_655
O21 Mo1 O2 84.4(8) . .
O5 Mo1 O2 168.6(8) . .
O3 Mo1 O2 80.5(8) . .
O13 Mo1 O2 73.5(8) . .
O12 Mo1 O2 71.5(7) 1_655 .
O21 Mo1 Mo2 132.4(6) . 1_655
O5 Mo1 Mo2 89.8(7) . 1_655
O3 Mo1 Mo2 39.6(6) . 1_655
O13 Mo1 Mo2 125.7(5) . 1_655
O12 Mo1 Mo2 39.6(5) 1_655 1_655
O2 Mo1 Mo2 84.8(5) . 1_655
O21 Mo1 K1 149.6(6) . 2_656
O5 Mo1 K1 80.0(6) . 2_656
O3 Mo1 K1 115.4(6) . 2_656
O13 Mo1 K1 54.9(5) . 2_656
O12 Mo1 K1 41.1(5) 1_655 2_656
O2 Mo1 K1 89.0(5) . 2_656
Mo2 Mo1 K1 76.16(12) 1_655 2_656
O21 Mo1 K1 74.4(7) . .
O5 Mo1 K1 35.7(7) . .
O3 Mo1 K1 118.3(6) . .
O13 Mo1 K1 89.7(6) . .
O12 Mo1 K1 131.1(6) 1_655 .
O2 Mo1 K1 151.8(5) . .
Mo2 Mo1 K1 123.25(12) 1_655 .
K1 Mo1 K1 99.84(15) 2_656 .
O15 Mo2 O6 100.4(10) . .
O15 Mo2 O9 103.0(9) . .
O6 Mo2 O9 101.6(9) . .
O15 Mo2 O12 99.6(9) . .
O6 Mo2 O12 153.9(9) . .
O9 Mo2 O12 90.1(8) . .
O15 Mo2 O3 90.6(9) . 1_455
O6 Mo2 O3 88.6(8) . 1_455
O9 Mo2 O3 161.1(8) . 1_455
O12 Mo2 O3 74.5(8) . 1_455
O15 Mo2 O4 167.7(8) . .
O6 Mo2 O4 83.4(8) . .
O9 Mo2 O4 87.5(8) . .
O12 Mo2 O4 73.7(8) . .
O3 Mo2 O4 77.7(8) 1_455 .
O15 Mo2 Mo1 83.7(7) . 1_455
O6 Mo2 Mo1 124.1(6) . 1_455
O9 Mo2 Mo1 132.1(6) . 1_455
O12 Mo2 Mo1 42.4(5) . 1_455
O3 Mo2 Mo1 35.5(6) 1_455 1_455
O4 Mo2 Mo1 84.5(5) . 1_455
O15 Mo2 K1 54.2(7) . .
O6 Mo2 K1 73.1(7) . .
O9 Mo2 K1 64.3(6) . .
O12 Mo2 K1 132.8(6) . .
O3 Mo2 K1 134.5(6) 1_455 .
O4 Mo2 K1 137.7(5) . .
Mo1 Mo2 K1 137.78(15) 1_455 .
O15 Mo2 Th2 141.4(7) . .
O6 Mo2 Th2 41.1(7) . .
O9 Mo2 Th2 86.5(6) . .
O12 Mo2 Th2 117.9(6) . .
O3 Mo2 Th2 90.9(6) 1_455 .
O4 Mo2 Th2 44.2(5) . .
Mo1 Mo2 Th2 117.43(5) 1_455 .
K1 Mo2 Th2 100.28(14) . .
O15 Mo2 Sr1 79.9(6) . .
O6 Mo2 Sr1 47.8(6) . .
O9 Mo2 Sr1 148.5(6) . .
O12 Mo2 Sr1 120.6(5) . .
O3 Mo2 Sr1 46.3(6) 1_455 .
O4 Mo2 Sr1 94.5(5) . .
Mo1 Mo2 Sr1 79.27(10) 1_455 .
K1 Mo2 Sr1 94.95(17) . .
Th2 Mo2 Sr1 73.65(9) . .
O18 Mo3 O24 104.1(10) . .
O18 Mo3 O4 96.9(10) . .
O24 Mo3 O4 96.9(9) . .
O18 Mo3 O1 101.8(10) . .
O24 Mo3 O1 95.2(10) . .
O4 Mo3 O1 154.4(9) . .
O18 Mo3 O2 99.9(9) . 1_455
O24 Mo3 O2 155.3(10) . 1_455
O4 Mo3 O2 85.7(8) . 1_455
O1 Mo3 O2 74.2(8) . 1_455
O18 Mo3 O12 169.5(9) . .
O24 Mo3 O12 82.8(9) . .
O4 Mo3 O12 74.2(8) . .
O1 Mo3 O12 85.2(8) . .
O2 Mo3 O12 74.3(8) 1_455 .
O18 Mo3 Mo4 94.6(8) . 1_455
O24 Mo3 Mo4 134.5(7) . 1_455
O4 Mo3 Mo4 121.9(6) . 1_455
O1 Mo3 Mo4 39.8(6) . 1_455
O2 Mo3 Mo4 36.2(6) 1_455 1_455
O12 Mo3 Mo4 85.8(5) . 1_455
O18 Mo3 K1 62.2(7) . 1_565
O24 Mo3 K1 47.5(7) . 1_565
O4 Mo3 K1 121.6(6) . 1_565
O1 Mo3 K1 82.9(6) . 1_565
O2 Mo3 K1 147.4(6) 1_455 1_565
O12 Mo3 K1 127.1(5) . 1_565
Mo4 Mo3 K1 114.17(12) 1_455 1_565
O18 Mo3 K1 148.0(7) . 2_556
O24 Mo3 K1 63.1(8) . 2_556
O4 Mo3 K1 113.2(6) . 2_556
O1 Mo3 K1 54.0(6) . 2_556
O2 Mo3 K1 93.2(6) 1_455 2_556
O12 Mo3 K1 42.3(5) . 2_556
Mo4 Mo3 K1 79.07(12) 1_455 2_556
K1 Mo3 K1 91.56(18) 1_565 2_556
O11 Mo4 O19 99.8(10) . .
O11 Mo4 O8 98.2(9) . .
O19 Mo4 O8 101.2(9) . .
O11 Mo4 O2 104.8(10) . .
O19 Mo4 O2 96.3(9) . .
O8 Mo4 O2 148.2(9) . .
O11 Mo4 O1 94.1(9) . 1_655
O19 Mo4 O1 164.9(9) . 1_655
O8 Mo4 O1 82.6(8) . 1_655
O2 Mo4 O1 74.1(8) . 1_655
O11 Mo4 O13 171.4(8) . .
O19 Mo4 O13 88.5(8) . .
O8 Mo4 O13 77.7(8) . .
O2 Mo4 O13 76.4(8) . .
O1 Mo4 O13 77.9(7) 1_655 .
O11 Mo4 Mo3 92.7(7) . 1_655
O19 Mo4 Mo3 136.3(7) . 1_655
O8 Mo4 Mo3 118.4(6) . 1_655
O2 Mo4 Mo3 40.0(6) . 1_655
O1 Mo4 Mo3 36.0(6) 1_655 1_655
O13 Mo4 Mo3 82.9(5) . 1_655
O11 Mo4 Th1 80.1(6) . 2_666
O19 Mo4 Th1 145.7(7) . 2_666
O8 Mo4 Th1 45.7(6) . 2_666
O2 Mo4 Th1 117.1(6) . 2_666
O1 Mo4 Th1 43.1(6) 1_655 2_666
O13 Mo4 Th1 91.7(4) . 2_666
Mo3 Mo4 Th1 77.63(4) 1_655 2_666
O11 Mo4 Th1 138.1(7) . .
O19 Mo4 Th1 84.5(7) . .
O8 Mo4 Th1 40.8(6) . .
O2 Mo4 Th1 116.2(6) . .
O1 Mo4 Th1 89.3(6) 1_655 .
O13 Mo4 Th1 39.8(5) . .
Mo3 Mo4 Th1 112.98(4) 1_655 .
Th1 Mo4 Th1 74.21(4) 2_666 .
O11 Mo4 K2 49.4(7) . 2
O19 Mo4 K2 51.9(7) . 2
O8 Mo4 K2 94.8(6) . 2
O2 Mo4 K2 116.9(6) . 2
O1 Mo4 K2 142.9(6) 1_655 2
O13 Mo4 K2 137.9(5) . 2
Mo3 Mo4 K2 134.18(16) 1_655 2
Th1 Mo4 K2 112.60(14) 2_666 2
Th1 Mo4 K2 112.75(16) . 2
O22 Mo5 O16 105.4(10) . .
O22 Mo5 O23 101.9(10) . .
O16 Mo5 O23 100.4(9) . .
O22 Mo5 O20 100.5(10) . .
O16 Mo5 O20 84.7(10) . .
O23 Mo5 O20 154.7(9) . .
O22 Mo5 O14 101.4(9) . .
O16 Mo5 O14 148.8(10) . .
O23 Mo5 O14 89.3(8) . .
O20 Mo5 O14 74.8(9) . .
O22 Mo5 O14 173.2(9) . 2_655
O16 Mo5 O14 81.4(9) . 2_655
O23 Mo5 O14 76.1(8) . 2_655
O20 Mo5 O14 80.3(8) . 2_655
O14 Mo5 O14 72.2(8) . 2_655
O22 Mo5 Mo6 92.4(8) . .
O16 Mo5 Mo6 122.3(8) . .
O23 Mo5 Mo6 129.3(6) . .
O20 Mo5 Mo6 37.8(6) . .
O14 Mo5 Mo6 40.0(6) . .
O14 Mo5 Mo6 84.2(5) 2_655 .
O22 Mo5 Sr1 80.8(8) . 1_655
O16 Mo5 Sr1 49.2(7) . 1_655
O23 Mo5 Sr1 147.9(6) . 1_655
O20 Mo5 Sr1 48.4(7) . 1_655
O14 Mo5 Sr1 121.9(6) . 1_655
O14 Mo5 Sr1 104.5(5) 2_655 1_655
Mo6 Mo5 Sr1 82.07(10) . 1_655
O17 Mo6 O10 98.2(9) . .
O17 Mo6 O7 100.2(9) . .
O10 Mo6 O7 101.1(9) . .
O17 Mo6 O20 97.0(9) . .
O10 Mo6 O20 156.9(9) . .
O7 Mo6 O20 93.2(9) . .
O17 Mo6 O14 103.7(9) . .
O10 Mo6 O14 87.5(9) . .
O7 Mo6 O14 153.2(8) . .
O20 Mo6 O14 72.1(9) . .
O17 Mo6 O23 175.8(8) . 2_655
O10 Mo6 O23 85.9(8) . 2_655
O7 Mo6 O23 79.7(7) . 2_655
O20 Mo6 O23 78.9(8) . 2_655
O14 Mo6 O23 75.6(8) . 2_655
O17 Mo6 Mo5 91.9(7) . .
O10 Mo6 Mo5 125.1(6) . .
O7 Mo6 Mo5 130.0(6) . .
O20 Mo6 Mo5 37.0(7) . .
O14 Mo6 Mo5 37.9(6) . .
O23 Mo6 Mo5 85.1(5) 2_655 .
O17 Mo6 Th2 138.2(7) . .
O10 Mo6 Th2 83.9(6) . .
O7 Mo6 Th2 39.4(6) . .
O20 Mo6 Th2 96.2(6) . .
O14 Mo6 Th2 118.2(6) . .
O23 Mo6 Th2 42.8(5) 2_655 .
Mo5 Mo6 Th2 121.05(5) . .
O17 Mo6 K2 49.3(7) . .
O10 Mo6 K2 52.1(6) . .
O7 Mo6 K2 91.6(6) . .
O20 Mo6 K2 146.2(6) . .
O14 Mo6 K2 113.2(6) . .
O23 Mo6 K2 134.9(5) 2_655 .
Mo5 Mo6 K2 130.19(16) . .
Th2 Mo6 K2 108.46(16) . .
O17 Mo6 K2 72.3(7) . 2_545
O10 Mo6 K2 122.1(6) . 2_545
O7 Mo6 K2 33.3(6) . 2_545
O20 Mo6 K2 79.2(7) . 2_545
O14 Mo6 K2 150.4(6) . 2_545
O23 Mo6 K2 106.3(5) 2_655 2_545
Mo5 Mo6 K2 112.48(13) . 2_545
Th2 Mo6 K2 71.52(14) . 2_545
K2 Mo6 K2 86.88(19) . 2_545
O17 Mo6 Sr1 24.9(7) . 2_545
O10 Mo6 Sr1 102.6(6) . 2_545
O7 Mo6 Sr1 122.4(6) . 2_545
O20 Mo6 Sr1 84.4(6) . 2_545
O14 Mo6 Sr1 79.4(6) . 2_545
O23 Mo6 Sr1 153.2(5) 2_655 2_545
Mo5 Mo6 Sr1 69.13(9) . 2_545
Th2 Mo6 Sr1 161.84(9) . 2_545
K2 Mo6 Sr1 64.98(17) . 2_545
K2 Mo6 Sr1 90.86(16) 2_545 2_545
Mo3 O1 Mo4 104.2(9) . 1_455
Mo3 O1 Th1 148.5(10) . 2_566
Mo4 O1 Th1 100.0(8) 1_455 2_566
Mo3 O1 K1 95.9(8) . 2_556
Mo4 O1 K1 117.5(8) 1_455 2_556
Th1 O1 K1 90.5(6) 2_566 2_556
Mo4 O2 Mo3 103.8(9) . 1_655
Mo4 O2 Mo1 100.5(9) . .
Mo3 O2 Mo1 105.1(9) 1_655 .
Mo1 O3 Mo2 104.8(9) . 1_655
Mo1 O3 Sr1 144.3(10) . 1_655
Mo2 O3 Sr1 99.4(8) 1_655 1_655
Mo3 O4 Mo2 108.6(9) . .
Mo3 O4 Th2 148.3(10) . .
Mo2 O4 Th2 99.1(7) . .
Mo1 O5 Th1 141.1(11) . 2_656
Mo1 O5 K1 123.3(10) . .
Th1 O5 K1 94.2(7) 2_656 .
Mo2 O6 Th2 111.0(9) . .
Mo2 O6 Sr1 103.7(9) . .
Th2 O6 Sr1 109.5(7) . .
Mo2 O6 K1 76.4(7) . .
Th2 O6 K1 131.1(7) . .
Sr1 O6 K1 115.5(7) . .
Mo6 O7 Th2 112.2(8) . .
Mo6 O7 K2 123.6(9) . 2_545
Th2 O7 K2 121.1(8) . 2_545
Mo4 O8 Th1 109.1(8) . .
Mo4 O8 Th1 102.2(8) . 2_666
Th1 O8 Th1 115.8(7) . 2_666
Mo4 O8 K1 131.7(10) . 1_565
Th1 O8 K1 101.0(7) . 1_565
Th1 O8 K1 97.3(6) 2_666 1_565
Mo2 O9 Th1 151.7(10) . .
Mo2 O9 K1 84.4(7) . .
Th1 O9 K1 122.2(7) . .
Mo6 O10 Th2 152.3(10) . 2
Mo6 O10 K2 97.7(8) . .
Th2 O10 K2 106.5(7) 2 .
Mo4 O11 Sr1 138.4(11) . 1_665
Mo4 O11 K2 102.5(9) . 2
Sr1 O11 K2 100.7(7) 1_665 2
Mo2 O12 Mo1 97.9(8) . 1_455
Mo2 O12 Mo3 100.8(8) . .
Mo1 O12 Mo3 109.1(8) 1_455 .
Mo2 O12 K1 136.7(9) . 2_556
Mo1 O12 K1 107.1(8) 1_455 2_556
Mo3 O12 K1 103.4(7) . 2_556
Mo1 O13 Mo4 105.8(8) . .
Mo1 O13 Th1 147.0(9) . .
Mo4 O13 Th1 102.7(7) . .
Mo1 O13 K1 95.3(7) . 2_656
Mo4 O13 K1 112.2(7) . 2_656
Th1 O13 K1 89.1(6) . 2_656
Mo5 O14 Mo6 102.1(9) . .
Mo5 O14 Mo5 107.8(8) . 2_655
Mo6 O14 Mo5 97.9(8) . 2_655
Mo2 O15 Th1 147.4(11) . 2_556
Mo2 O15 K1 94.5(9) . .
Th1 O15 K1 113.1(8) 2_556 .
Mo5 O16 Th2 144.7(13) . 1_655
Mo5 O16 Sr1 101.3(9) . 1_655
Th2 O16 Sr1 113.9(9) 1_655 1_655
Mo6 O17 Sr1 138.5(11) . 2_545
Mo6 O17 K2 102.8(9) . .
Sr1 O17 K2 100.2(7) 2_545 .
Mo3 O18 Sr1 130.9(11) . 1_565
Mo3 O18 K2 137.9(12) . 2
Sr1 O18 K2 88.5(7) 1_565 2
Mo3 O18 K1 90.2(8) . 1_565
Sr1 O18 K1 112.0(7) 1_565 1_565
K2 O18 K1 86.3(6) 2 1_565
Mo4 O19 Th2 148.1(11) . .
Mo4 O19 K2 98.7(9) . 2
Th2 O19 K2 103.8(7) . 2
Mo5 O20 Mo6 105.3(10) . .
Mo5 O20 Sr1 98.6(9) . 1_655
Mo6 O20 Sr1 140.1(10) . 1_655
Mo1 O21 Th2 153.4(10) . .
Mo5 O22 Sr1 134.0(12) . 2_545
Mo5 O22 K2 128.0(11) . 1_655
Sr1 O22 K2 96.3(7) 2_545 1_655
Mo5 O23 Mo6 108.3(9) . 2_655
Mo5 O23 Th2 148.6(10) . 2_655
Mo6 O23 Th2 96.9(7) 2_655 2_655
Mo3 O24 Th1 150.1(12) . .
Mo3 O24 K1 104.6(10) . 1_565
Th1 O24 K1 99.2(7) . 1_565
O17 Sr1 O11 128.4(7) 2_545 1_445
O17 Sr1 O3 152.8(7) 2_545 1_455
O11 Sr1 O3 75.2(7) 1_445 1_455
O17 Sr1 O22 78.4(7) 2_545 2_545
O11 Sr1 O22 68.0(7) 1_445 2_545
O3 Sr1 O22 127.5(7) 1_455 2_545
O17 Sr1 O20 108.7(7) 2_545 1_455
O11 Sr1 O20 104.1(7) 1_445 1_455
O3 Sr1 O20 72.0(7) 1_455 1_455
O22 Sr1 O20 81.9(7) 2_545 1_455
O17 Sr1 O16 82.2(7) 2_545 1_455
O11 Sr1 O16 149.2(7) 1_445 1_455
O3 Sr1 O16 76.2(6) 1_455 1_455
O22 Sr1 O16 123.5(7) 2_545 1_455
O20 Sr1 O16 55.4(7) 1_455 1_455
O17 Sr1 O6 95.8(6) 2_545 .
O11 Sr1 O6 110.6(6) 1_445 .
O3 Sr1 O6 59.7(6) 1_455 .
O22 Sr1 O6 169.9(7) 2_545 .
O20 Sr1 O6 108.0(6) 1_455 .
O16 Sr1 O6 63.2(6) 1_455 .
O17 Sr1 O18 72.0(7) 2_545 1_545
O11 Sr1 O18 77.6(7) 1_445 1_545
O3 Sr1 O18 105.7(6) 1_455 1_545
O22 Sr1 O18 101.5(7) 2_545 1_545
O20 Sr1 O18 176.5(7) 1_455 1_545
O16 Sr1 O18 121.7(7) 1_455 1_545
O6 Sr1 O18 68.6(6) . 1_545
O17 Sr1 Mo5 81.9(5) 2_545 1_455
O11 Sr1 Mo5 137.0(5) 1_445 1_455
O3 Sr1 Mo5 87.2(5) 1_455 1_455
O22 Sr1 Mo5 95.0(5) 2_545 1_455
O20 Sr1 Mo5 33.0(5) 1_455 1_455
O16 Sr1 Mo5 29.5(5) 1_455 1_455
O6 Sr1 Mo5 92.4(5) . 1_455
O18 Sr1 Mo5 145.3(5) 1_545 1_455
O17 Sr1 Mo2 123.9(5) 2_545 .
O11 Sr1 Mo2 86.9(5) 1_445 .
O3 Sr1 Mo2 34.3(4) 1_455 .
O22 Sr1 Mo2 154.4(6) 2_545 .
O20 Sr1 Mo2 99.9(5) 1_455 .
O16 Sr1 Mo2 75.9(5) 1_455 .
O6 Sr1 Mo2 28.5(4) . .
O18 Sr1 Mo2 77.1(4) 1_545 .
Mo5 Sr1 Mo2 100.26(14) 1_455 .
O17 Sr1 Mo6 16.6(4) 2_545 2_545
O11 Sr1 Mo6 113.0(5) 1_445 2_545
O3 Sr1 Mo6 168.7(5) 1_455 2_545
O22 Sr1 Mo6 63.7(5) 2_545 2_545
O20 Sr1 Mo6 111.8(5) 1_455 2_545
O16 Sr1 Mo6 97.0(5) 1_455 2_545
O6 Sr1 Mo6 109.3(5) . 2_545
O18 Sr1 Mo6 69.8(4) 1_545 2_545
Mo5 Sr1 Mo6 91.19(12) 1_455 2_545
Mo2 Sr1 Mo6 135.64(16) . 2_545
O17 Sr1 K2 42.1(5) 2_545 2_545
O11 Sr1 K2 123.5(5) 1_445 2_545
O3 Sr1 K2 116.7(5) 1_455 2_545
O22 Sr1 K2 114.6(6) 2_545 2_545
O20 Sr1 K2 132.4(5) 1_455 2_545
O16 Sr1 K2 80.2(5) 1_455 2_545
O6 Sr1 K2 57.2(4) . 2_545
O18 Sr1 K2 45.9(5) 1_545 2_545
Mo5 Sr1 K2 99.44(17) 1_455 2_545
Mo2 Sr1 K2 83.20(16) . 2_545
Mo6 Sr1 K2 52.56(14) 2_545 2_545
O12 K1 O8 116.9(7) 2_556 1_545
O12 K1 O15 80.9(6) 2_556 .
O8 K1 O15 151.2(6) 1_545 .
O12 K1 O5 99.9(6) 2_556 .
O8 K1 O5 69.6(6) 1_545 .
O15 K1 O5 132.5(7) . .
O12 K1 O24 105.2(7) 2_556 1_545
O8 K1 O24 62.5(7) 1_545 1_545
O15 K1 O24 91.9(7) . 1_545
O5 K1 O24 131.9(7) . 1_545
O12 K1 O9 74.8(6) 2_556 .
O8 K1 O9 146.6(6) 1_545 .
O15 K1 O9 56.5(6) . .
O5 K1 O9 77.7(6) . .
O24 K1 O9 148.3(7) 1_545 .
O12 K1 O1 57.7(6) 2_556 2_556
O8 K1 O1 66.5(6) 1_545 2_556
O15 K1 O1 112.6(6) . 2_556
O5 K1 O1 107.1(6) . 2_556
O24 K1 O1 57.9(6) 1_545 2_556
O9 K1 O1 132.5(6) . 2_556
O12 K1 O13 55.9(5) 2_556 2_656
O8 K1 O13 67.4(5) 1_545 2_656
O15 K1 O13 136.4(6) . 2_656
O5 K1 O13 59.3(5) . 2_656
O24 K1 O13 103.9(6) 1_545 2_656
O9 K1 O13 101.9(5) . 2_656
O1 K1 O13 51.2(5) 2_556 2_656
O12 K1 O18 137.4(6) 2_556 1_545
O8 K1 O18 87.2(6) 1_545 1_545
O15 K1 O18 65.7(6) . 1_545
O5 K1 O18 122.0(6) . 1_545
O24 K1 O18 53.2(6) 1_545 1_545
O9 K1 O18 104.9(6) . 1_545
O1 K1 O18 110.8(6) 2_556 1_545
O13 K1 O18 152.8(6) 2_656 1_545
O12 K1 O6 120.4(6) 2_556 .
O8 K1 O6 121.7(6) 1_545 .
O15 K1 O6 51.9(6) . .
O5 K1 O6 90.8(6) . .
O24 K1 O6 109.9(6) 1_545 .
O9 K1 O6 50.5(5) . .
O1 K1 O6 162.2(6) 2_556 .
O13 K1 O6 145.1(6) 2_656 .
O18 K1 O6 57.1(5) 1_545 .
O12 K1 Mo2 90.3(5) 2_556 .
O8 K1 Mo2 152.2(5) 1_545 .
O15 K1 Mo2 31.3(4) . .
O5 K1 Mo2 101.6(5) . .
O24 K1 Mo2 118.3(5) 1_545 .
O9 K1 Mo2 31.3(4) . .
O1 K1 Mo2 139.8(5) 2_556 .
O13 K1 Mo2 132.1(4) 2_656 .
O18 K1 Mo2 75.1(4) 1_545 .
O6 K1 Mo2 30.5(4) . .
O12 K1 Mo3 117.7(5) 2_556 1_545
O8 K1 Mo3 80.6(4) 1_545 1_545
O15 K1 Mo3 70.9(4) . 1_545
O5 K1 Mo3 139.8(5) . 1_545
O24 K1 Mo3 27.8(4) 1_545 1_545
O9 K1 Mo3 123.6(4) . 1_545
O1 K1 Mo3 83.7(4) 2_556 1_545
O13 K1 Mo3 131.7(4) 2_656 1_545
O18 K1 Mo3 27.6(4) 1_545 1_545
O6 K1 Mo3 82.4(4) . 1_545
Mo2 K1 Mo3 92.27(18) . 1_545
O7 K2 O17 76.6(6) 2_545 .
O7 K2 O11 110.0(7) 2_545 2
O17 K2 O11 173.2(7) . 2
O7 K2 O10 123.7(6) 2_545 .
O17 K2 O10 56.6(6) . .
O11 K2 O10 116.8(6) 2 .
O7 K2 O19 166.7(7) 2_545 2
O17 K2 O19 116.6(6) . 2
O11 K2 O19 56.8(6) 2 2
O10 K2 O19 66.8(6) . 2
O7 K2 O22 95.9(7) 2_545 1_455
O17 K2 O22 116.6(7) . 1_455
O11 K2 O22 61.6(6) 2 1_455
O10 K2 O22 80.9(6) . 1_455
O19 K2 O22 76.8(7) 2 1_455
O7 K2 O18 116.7(7) 2_545 2
O17 K2 O18 68.5(6) . 2
O11 K2 O18 109.1(7) 2 2
O10 K2 O18 75.7(6) . 2
O19 K2 O18 72.4(7) 2 2
O22 K2 O18 146.7(7) 1_455 2
O7 K2 Mo6 95.9(5) 2_545 .
O17 K2 Mo6 28.0(4) . .
O11 K2 Mo6 146.0(5) 2 .
O10 K2 Mo6 30.1(4) . .
O19 K2 Mo6 95.8(4) 2 .
O22 K2 Mo6 95.0(5) 1_455 .
O18 K2 Mo6 76.3(4) 2 .
O7 K2 Mo4 137.7(5) 2_545 2
O17 K2 Mo4 145.6(5) . 2
O11 K2 Mo4 28.1(5) 2 2
O10 K2 Mo4 94.5(4) . 2
O19 K2 Mo4 29.4(4) 2 2
O22 K2 Mo4 70.7(5) 1_455 2
O18 K2 Mo4 87.7(5) 2 2
Mo6 K2 Mo4 124.5(2) . 2
O7 K2 Mo6 23.1(4) 2_545 2_545
O17 K2 Mo6 83.2(5) . 2_545
O11 K2 Mo6 102.1(5) 2 2_545
O10 K2 Mo6 114.0(5) . 2_545
O19 K2 Mo6 149.4(5) 2 2_545
O22 K2 Mo6 73.3(5) 1_455 2_545
O18 K2 Mo6 138.3(5) 2 2_545
Mo6 K2 Mo6 93.12(19) . 2_545
Mo4 K2 Mo6 129.1(2) 2 2_545
O7 K2 Sr1 74.8(5) 2_545 2_545
O17 K2 Sr1 37.8(4) . 2_545
O11 K2 Sr1 144.6(5) 2 2_545
O10 K2 Sr1 84.1(4) . 2_545
O19 K2 Sr1 116.5(5) 2 2_545
O22 K2 Sr1 153.7(5) 1_455 2_545
O18 K2 Sr1 45.5(5) 2 2_545
Mo6 K2 Sr1 62.45(15) . 2_545
Mo4 K2 Sr1 132.2(3) 2 2_545
Mo6 K2 Sr1 93.58(19) 2_545 2_545
O7 K2 Sr1 81.5(5) 2_545 2_445
O17 K2 Sr1 145.4(5) . 2_445
O11 K2 Sr1 37.5(5) 2 2_445
O10 K2 Sr1 119.6(5) . 2_445
O19 K2 Sr1 85.8(5) 2 2_445
O22 K2 Sr1 39.7(4) 1_455 2_445
O18 K2 Sr1 146.0(5) 2 2_445
Mo6 K2 Sr1 133.1(3) . 2_445
Mo4 K2 Sr1 62.33(15) 2 2_445
Mo6 K2 Sr1 66.92(16) 2_545 2_445
Sr1 K2 Sr1 153.5(3) 2_545 2_445
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Th1 O24 2.34(2) .
Th1 O13 2.351(19) .
Th1 O9 2.393(18) .
Th1 O15 2.41(2) 2_556
Th1 O1 2.42(2) 2_566
Th1 O8 2.48(2) .
Th1 O5 2.51(2) 2_656
Th1 O8 2.557(19) 2_666
Th1 Mo4 3.4906(18) 2_666
Th1 Mo4 3.5812(18) .
Th1 K1 3.941(8) 2_656
Th1 K1 3.992(8) 1_565
Th2 O10 2.35(2) 2
Th2 O16 2.39(2) 1_455
Th2 O19 2.42(2) .
Th2 O23 2.43(2) 2_655
Th2 O7 2.439(18) .
Th2 O21 2.482(19) .
Th2 O6 2.51(2) .
Th2 O4 2.518(19) .
Th2 Mo6 3.5543(17) .
Th2 Mo2 3.5641(17) .
Th2 K2 4.183(8) 2
Th2 Sr1 4.316(6) .
Mo1 O21 1.749(18) .
Mo1 O5 1.76(2) .
Mo1 O3 1.89(2) .
Mo1 O13 1.943(18) .
Mo1 O12 2.145(19) 1_655
Mo1 O2 2.37(2) .
Mo1 Mo2 3.1493(17) 1_655
Mo1 K1 3.896(8) 2_656
Mo1 K1 4.099(8) .
Mo2 O15 1.78(2) .
Mo2 O6 1.79(2) .
Mo2 O9 1.786(18) .
Mo2 O12 2.029(19) .
Mo2 O3 2.078(19) 1_455
Mo2 O4 2.15(2) .
Mo2 Mo1 3.1492(17) 1_455
Mo2 K1 3.417(8) .
Mo2 Sr1 3.635(6) .
Mo3 O18 1.75(2) .
Mo3 O24 1.82(2) .
Mo3 O4 1.898(19) .
Mo3 O1 1.95(2) .
Mo3 O2 2.13(2) 1_455
Mo3 O12 2.24(2) .
Mo3 Mo4 3.2189(17) 1_455
Mo3 K1 3.782(8) 1_565
Mo3 K1 3.873(8) 2_556
Mo4 O11 1.75(2) .
Mo4 O19 1.80(2) .
Mo4 O8 1.897(19) .
Mo4 O2 1.96(2) .
Mo4 O1 2.13(2) 1_655
Mo4 O13 2.234(19) .
Mo4 Mo3 3.2189(17) 1_655
Mo4 Th1 3.4905(18) 2_666
Mo4 K2 3.621(8) 2
Mo5 O22 1.79(2) .
Mo5 O16 1.79(2) .
Mo5 O23 1.89(2) .
Mo5 O20 1.97(2) .
Mo5 O14 1.99(2) .
Mo5 O14 2.44(2) 2_655
Mo5 Mo6 3.1595(17) .
Mo5 Sr1 3.573(6) 1_655
Mo6 O17 1.721(19) .
Mo6 O10 1.814(19) .
Mo6 O7 1.823(19) .
Mo6 O20 2.01(2) .
Mo6 O14 2.08(2) .
Mo6 O23 2.313(18) 2_655
Mo6 K2 3.581(8) .
Mo6 K2 3.871(9) 2_545
Mo6 Sr1 3.998(6) 2_545
O1 Mo4 2.13(2) 1_455
O1 Th1 2.42(2) 2_566
O1 K1 3.15(2) 2_556
O2 Mo3 2.13(2) 1_655
O3 Mo2 2.078(19) 1_655
O3 Sr1 2.66(2) 1_655
O5 Th1 2.51(2) 2_656
O5 K1 2.86(2) .
O6 Sr1 2.77(2) .
O6 K1 3.36(2) .
O7 K2 2.55(2) 2_545
O8 Th1 2.557(18) 2_666
O8 K1 2.69(2) 1_565
O9 K1 3.09(2) .
O10 Th2 2.35(2) 2
O10 K2 2.85(2) .
O11 Sr1 2.57(2) 1_665
O11 K2 2.82(2) 2
O12 Mo1 2.145(18) 1_455
O12 K1 2.68(2) 2_556
O13 K1 3.201(19) 2_656
O14 Mo5 2.44(2) 2_655
O15 Th1 2.41(2) 2_556
O15 K1 2.78(2) .
O16 Th2 2.39(2) 1_655
O16 Sr1 2.76(2) 1_655
O17 Sr1 2.54(2) 2_545
O17 K2 2.78(2) .
O18 Sr1 2.92(2) 1_565
O18 K2 2.94(3) 2
O18 K1 3.35(2) 1_565
O19 K2 2.88(2) 2
O20 Sr1 2.70(2) 1_655
O22 Sr1 2.67(2) 2_545
O22 K2 2.91(3) 1_655
O23 Mo6 2.313(18) 2_655
O23 Th2 2.43(2) 2_655
O24 K1 2.88(2) 1_565
Sr1 O17 2.54(2) 2_545
Sr1 O11 2.57(2) 1_445
Sr1 O3 2.66(2) 1_455
Sr1 O22 2.67(2) 2_545
Sr1 O20 2.70(2) 1_455
Sr1 O16 2.76(2) 1_455
Sr1 O18 2.92(2) 1_545
Sr1 Mo5 3.573(6) 1_455
Sr1 Mo6 3.998(6) 2_545
Sr1 K2 4.087(10) 2_545
K1 O12 2.68(2) 2_556
K1 O8 2.69(2) 1_545
K1 O24 2.88(2) 1_545
K1 O1 3.15(2) 2_556
K1 O13 3.201(19) 2_656
K1 O18 3.35(2) 1_545
K1 Mo3 3.782(8) 1_545
K2 O7 2.55(2) 2_545
K2 O11 2.82(2) 2
K2 O19 2.88(2) 2
K2 O22 2.91(3) 1_455
K2 O18 2.94(3) 2
K2 Mo4 3.621(8) 2
K2 Mo6 3.871(9) 2_545
K2 Sr1 4.087(10) 2_545
K2 Sr1 4.153(10) 2_445
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O10 Th2 Mo2 O15 141.7(12) 2 .
O16 Th2 Mo2 O15 73.3(12) 1_455 .
O19 Th2 Mo2 O15 -137.4(12) . .
O23 Th2 Mo2 O15 -73.1(16) 2_655 .
O7 Th2 Mo2 O15 1.7(11) . .
O21 Th2 Mo2 O15 -66.3(11) . .
O6 Th2 Mo2 O15 5.4(14) . .
O4 Th2 Mo2 O15 163.4(13) . .
Mo6 Th2 Mo2 O15 -0.3(10) . .
K2 Th2 Mo2 O15 -174.2(10) 2 .
Sr1 Th2 Mo2 O15 48.7(10) . .
O10 Th2 Mo2 O6 136.2(11) 2 .
O16 Th2 Mo2 O6 67.9(11) 1_455 .
O19 Th2 Mo2 O6 -142.8(11) . .
O23 Th2 Mo2 O6 -78.6(16) 2_655 .
O7 Th2 Mo2 O6 -3.7(10) . .
O21 Th2 Mo2 O6 -71.7(10) . .
O4 Th2 Mo2 O6 158.0(12) . .
Mo6 Th2 Mo2 O6 -5.7(9) . .
K2 Th2 Mo2 O6 -179.6(10) 2 .
Sr1 Th2 Mo2 O6 43.2(9) . .
O10 Th2 Mo2 O9 -111.7(8) 2 .
O16 Th2 Mo2 O9 179.9(8) 1_455 .
O19 Th2 Mo2 O9 -30.8(8) . .
O23 Th2 Mo2 O9 33.5(14) 2_655 .
O7 Th2 Mo2 O9 108.3(8) . .
O21 Th2 Mo2 O9 40.3(8) . .
O6 Th2 Mo2 O9 112.0(11) . .
O4 Th2 Mo2 O9 -90.0(9) . .
Mo6 Th2 Mo2 O9 106.3(6) . .
K2 Th2 Mo2 O9 -67.6(6) 2 .
Sr1 Th2 Mo2 O9 155.3(6) . .
O10 Th2 Mo2 O12 -23.5(8) 2 .
O16 Th2 Mo2 O12 -91.8(8) 1_455 .
O19 Th2 Mo2 O12 57.5(8) . .
O23 Th2 Mo2 O12 121.7(14) 2_655 .
O7 Th2 Mo2 O12 -163.4(7) . .
O21 Th2 Mo2 O12 128.5(7) . .
O6 Th2 Mo2 O12 -159.7(11) . .
O4 Th2 Mo2 O12 -1.7(9) . .
Mo6 Th2 Mo2 O12 -165.4(6) . .
K2 Th2 Mo2 O12 20.7(6) 2 .
Sr1 Th2 Mo2 O12 -116.5(6) . .
O10 Th2 Mo2 O3 49.5(7) 2 1_455
O16 Th2 Mo2 O3 -18.9(8) 1_455 1_455
O19 Th2 Mo2 O3 130.4(7) . 1_455
O23 Th2 Mo2 O3 -165.3(14) 2_655 1_455
O7 Th2 Mo2 O3 -90.5(7) . 1_455
O21 Th2 Mo2 O3 -158.5(7) . 1_455
O6 Th2 Mo2 O3 -86.8(11) . 1_455
O4 Th2 Mo2 O3 71.3(9) . 1_455
Mo6 Th2 Mo2 O3 -92.5(6) . 1_455
K2 Th2 Mo2 O3 93.7(6) 2 1_455
Sr1 Th2 Mo2 O3 -43.5(6) . 1_455
O10 Th2 Mo2 O4 -21.8(9) 2 .
O16 Th2 Mo2 O4 -90.1(9) 1_455 .
O19 Th2 Mo2 O4 59.2(9) . .
O23 Th2 Mo2 O4 123.4(15) 2_655 .
O7 Th2 Mo2 O4 -161.7(8) . .
O21 Th2 Mo2 O4 130.2(8) . .
O6 Th2 Mo2 O4 -158.0(12) . .
Mo6 Th2 Mo2 O4 -163.7(7) . .
K2 Th2 Mo2 O4 22.4(7) 2 .
Sr1 Th2 Mo2 O4 -114.8(7) . .
O10 Th2 Mo2 Mo1 24.8(5) 2 1_455
O16 Th2 Mo2 Mo1 -43.6(6) 1_455 1_455
O19 Th2 Mo2 Mo1 105.7(5) . 1_455
O23 Th2 Mo2 Mo1 170.0(13) 2_655 1_455
O7 Th2 Mo2 Mo1 -115.2(4) . 1_455
O21 Th2 Mo2 Mo1 176.8(4) . 1_455
O6 Th2 Mo2 Mo1 -111.5(9) . 1_455
O4 Th2 Mo2 Mo1 46.5(7) . 1_455
Mo6 Th2 Mo2 Mo1 -117.19(7) . 1_455
K2 Th2 Mo2 Mo1 68.94(13) 2 1_455
Sr1 Th2 Mo2 Mo1 -68.23(11) . 1_455
O10 Th2 Mo2 K1 -174.8(5) 2 .
O16 Th2 Mo2 K1 116.8(6) 1_455 .
O19 Th2 Mo2 K1 -93.8(5) . .
O23 Th2 Mo2 K1 -29.6(13) 2_655 .
O7 Th2 Mo2 K1 45.2(5) . .
O21 Th2 Mo2 K1 -22.8(5) . .
O6 Th2 Mo2 K1 48.9(10) . .
O4 Th2 Mo2 K1 -153.0(7) . .
Mo6 Th2 Mo2 K1 43.23(15) . .
K2 Th2 Mo2 K1 -130.64(18) 2 .
Sr1 Th2 Mo2 K1 92.18(17) . .
O10 Th2 Mo2 Sr1 93.0(5) 2 .
O16 Th2 Mo2 Sr1 24.6(6) 1_455 .
O19 Th2 Mo2 Sr1 174.0(5) . .
O23 Th2 Mo2 Sr1 -121.8(13) 2_655 .
O7 Th2 Mo2 Sr1 -47.0(4) . .
O21 Th2 Mo2 Sr1 -115.0(4) . .
O6 Th2 Mo2 Sr1 -43.2(9) . .
O4 Th2 Mo2 Sr1 114.8(7) . .
Mo6 Th2 Mo2 Sr1 -48.96(11) . .
K2 Th2 Mo2 Sr1 137.17(15) 2 .
O24 Th1 Mo4 O11 55.4(11) . .
O13 Th1 Mo4 O11 -167.2(12) . .
O9 Th1 Mo4 O11 127.1(11) . .
O15 Th1 Mo4 O11 109(2) 2_556 .
O1 Th1 Mo4 O11 -15.9(11) 2_566 .
O8 Th1 Mo4 O11 -15.8(13) . .
O5 Th1 Mo4 O11 -144.1(11) 2_656 .
O8 Th1 Mo4 O11 -72.3(11) 2_666 .
Mo4 Th1 Mo4 O11 -54.4(10) 2_666 .
K1 Th1 Mo4 O11 -115.9(10) 2_656 .
K1 Th1 Mo4 O11 10.6(10) 1_565 .
O24 Th1 Mo4 O19 -43.1(9) . .
O13 Th1 Mo4 O19 94.4(9) . .
O9 Th1 Mo4 O19 28.7(8) . .
O15 Th1 Mo4 O19 11(2) 2_556 .
O1 Th1 Mo4 O19 -114.3(8) 2_566 .
O8 Th1 Mo4 O19 -114.3(11) . .
O5 Th1 Mo4 O19 117.5(8) 2_656 .
O8 Th1 Mo4 O19 -170.8(8) 2_666 .
Mo4 Th1 Mo4 O19 -152.8(7) 2_666 .
K1 Th1 Mo4 O19 145.6(7) 2_656 .
K1 Th1 Mo4 O19 -87.8(7) 1_565 .
O24 Th1 Mo4 O8 71.2(10) . .
O13 Th1 Mo4 O8 -151.3(11) . .
O9 Th1 Mo4 O8 143.0(10) . .
O15 Th1 Mo4 O8 125(2) 2_556 .
O1 Th1 Mo4 O8 -0.1(10) 2_566 .
O5 Th1 Mo4 O8 -128.2(10) 2_656 .
O8 Th1 Mo4 O8 -56.5(12) 2_666 .
Mo4 Th1 Mo4 O8 -38.6(9) 2_666 .
K1 Th1 Mo4 O8 -100.1(9) 2_656 .
K1 Th1 Mo4 O8 26.5(9) 1_565 .
O24 Th1 Mo4 O2 -137.4(8) . .
O13 Th1 Mo4 O2 0.1(10) . .
O9 Th1 Mo4 O2 -65.6(8) . .
O15 Th1 Mo4 O2 -84(2) 2_556 .
O1 Th1 Mo4 O2 151.3(8) 2_566 .
O8 Th1 Mo4 O2 151.4(11) . .
O5 Th1 Mo4 O2 23.1(8) 2_656 .
O8 Th1 Mo4 O2 94.9(8) 2_666 .
Mo4 Th1 Mo4 O2 112.8(7) 2_666 .
K1 Th1 Mo4 O2 51.3(7) 2_656 .
K1 Th1 Mo4 O2 177.9(7) 1_565 .
O24 Th1 Mo4 O1 150.7(8) . 1_655
O13 Th1 Mo4 O1 -71.8(9) . 1_655
O9 Th1 Mo4 O1 -137.5(7) . 1_655
O15 Th1 Mo4 O1 -155.6(19) 2_556 1_655
O1 Th1 Mo4 O1 79.5(9) 2_566 1_655
O8 Th1 Mo4 O1 79.5(10) . 1_655
O5 Th1 Mo4 O1 -48.7(7) 2_656 1_655
O8 Th1 Mo4 O1 23.0(7) 2_666 1_655
Mo4 Th1 Mo4 O1 41.0(6) 2_666 1_655
K1 Th1 Mo4 O1 -20.6(6) 2_656 1_655
K1 Th1 Mo4 O1 106.0(6) 1_565 1_655
O24 Th1 Mo4 O13 -137.4(9) . .
O9 Th1 Mo4 O13 -65.7(8) . .
O15 Th1 Mo4 O13 -84(2) 2_556 .
O1 Th1 Mo4 O13 151.3(9) 2_566 .
O8 Th1 Mo4 O13 151.3(11) . .
O5 Th1 Mo4 O13 23.1(8) 2_656 .
O8 Th1 Mo4 O13 94.8(8) 2_666 .
Mo4 Th1 Mo4 O13 112.8(7) 2_666 .
K1 Th1 Mo4 O13 51.2(7) 2_656 .
K1 Th1 Mo4 O13 177.8(7) 1_565 .
O24 Th1 Mo4 Mo3 178.6(5) . 1_655
O13 Th1 Mo4 Mo3 -44.0(7) . 1_655
O9 Th1 Mo4 Mo3 -109.7(5) . 1_655
O15 Th1 Mo4 Mo3 -127.8(19) 2_556 1_655
O1 Th1 Mo4 Mo3 107.3(5) 2_566 1_655
O8 Th1 Mo4 Mo3 107.4(9) . 1_655
O5 Th1 Mo4 Mo3 -20.9(5) 2_656 1_655
O8 Th1 Mo4 Mo3 50.9(5) 2_666 1_655
Mo4 Th1 Mo4 Mo3 68.80(5) 2_666 1_655
K1 Th1 Mo4 Mo3 7.25(13) 2_656 1_655
K1 Th1 Mo4 Mo3 133.82(13) 1_565 1_655
O24 Th1 Mo4 Th1 109.8(5) . 2_666
O13 Th1 Mo4 Th1 -112.8(7) . 2_666
O9 Th1 Mo4 Th1 -178.5(5) . 2_666
O15 Th1 Mo4 Th1 163.4(19) 2_556 2_666
O1 Th1 Mo4 Th1 38.5(5) 2_566 2_666
O8 Th1 Mo4 Th1 38.6(9) . 2_666
O5 Th1 Mo4 Th1 -89.7(5) 2_656 2_666
O8 Th1 Mo4 Th1 -17.9(5) 2_666 2_666
Mo4 Th1 Mo4 Th1 0.000(2) 2_666 2_666
K1 Th1 Mo4 Th1 -61.54(12) 2_656 2_666
K1 Th1 Mo4 Th1 65.02(12) 1_565 2_666
O24 Th1 Mo4 K2 1.4(5) . 2
O13 Th1 Mo4 K2 138.9(7) . 2
O9 Th1 Mo4 K2 73.2(5) . 2
O15 Th1 Mo4 K2 55.1(19) 2_556 2
O1 Th1 Mo4 K2 -69.8(5) 2_566 2
O8 Th1 Mo4 K2 -69.8(9) . 2
O5 Th1 Mo4 K2 162.0(5) 2_656 2
O8 Th1 Mo4 K2 -126.3(5) 2_666 2
Mo4 Th1 Mo4 K2 -108.33(15) 2_666 2
K1 Th1 Mo4 K2 -169.87(19) 2_656 2
K1 Th1 Mo4 K2 -43.31(19) 1_565 2
O22 Mo5 Mo6 O17 5.0(10) . .
O16 Mo5 Mo6 O17 -104.9(11) . .
O23 Mo5 Mo6 O17 112.5(10) . .
O20 Mo5 Mo6 O17 -99.1(13) . .
O14 Mo5 Mo6 O17 110.0(11) . .
O14 Mo5 Mo6 O17 179.2(8) 2_655 .
Sr1 Mo5 Mo6 O17 -75.3(7) 1_655 .
O22 Mo5 Mo6 O10 -96.3(11) . .
O16 Mo5 Mo6 O10 153.8(11) . .
O23 Mo5 Mo6 O10 11.1(10) . .
O20 Mo5 Mo6 O10 159.5(13) . .
O14 Mo5 Mo6 O10 8.7(12) . .
O14 Mo5 Mo6 O10 77.8(9) 2_655 .
Sr1 Mo5 Mo6 O10 -176.7(7) 1_655 .
O22 Mo5 Mo6 O7 110.1(11) . .
O16 Mo5 Mo6 O7 0.2(11) . .
O23 Mo5 Mo6 O7 -142.4(10) . .
O20 Mo5 Mo6 O7 5.9(13) . .
O14 Mo5 Mo6 O7 -144.9(12) . .
O14 Mo5 Mo6 O7 -75.8(9) 2_655 .
Sr1 Mo5 Mo6 O7 29.8(7) 1_655 .
O22 Mo5 Mo6 O20 104.1(13) . .
O16 Mo5 Mo6 O20 -5.8(13) . .
O23 Mo5 Mo6 O20 -148.4(13) . .
O14 Mo5 Mo6 O20 -150.8(14) . .
O14 Mo5 Mo6 O20 -81.7(12) 2_655 .
Sr1 Mo5 Mo6 O20 23.8(11) 1_655 .
O22 Mo5 Mo6 O14 -105.0(12) . .
O16 Mo5 Mo6 O14 145.1(13) . .
O23 Mo5 Mo6 O14 2.5(12) . .
O20 Mo5 Mo6 O14 150.8(14) . .
O14 Mo5 Mo6 O14 69.2(12) 2_655 .
Sr1 Mo5 Mo6 O14 174.7(9) 1_655 .
O22 Mo5 Mo6 O23 -177.8(9) . 2_655
O16 Mo5 Mo6 O23 72.3(10) . 2_655
O23 Mo5 Mo6 O23 -70.3(10) . 2_655
O20 Mo5 Mo6 O23 78.0(12) . 2_655
O14 Mo5 Mo6 O23 -72.8(10) . 2_655
O14 Mo5 Mo6 O23 -3.7(7) 2_655 2_655
Sr1 Mo5 Mo6 O23 101.8(5) 1_655 2_655
O22 Mo5 Mo6 Th2 157.9(8) . .
O16 Mo5 Mo6 Th2 48.0(9) . .
O23 Mo5 Mo6 Th2 -94.6(7) . .
O20 Mo5 Mo6 Th2 53.7(11) . .
O14 Mo5 Mo6 Th2 -97.1(9) . .
O14 Mo5 Mo6 Th2 -27.9(5) 2_655 .
Sr1 Mo5 Mo6 Th2 77.57(10) 1_655 .
O22 Mo5 Mo6 K2 -29.2(8) . .
O16 Mo5 Mo6 K2 -139.1(9) . .
O23 Mo5 Mo6 K2 78.3(7) . .
O20 Mo5 Mo6 K2 -133.3(11) . .
O14 Mo5 Mo6 K2 75.8(9) . .
O14 Mo5 Mo6 K2 145.0(5) 2_655 .
Sr1 Mo5 Mo6 K2 -109.5(2) 1_655 .
O22 Mo5 Mo6 K2 76.6(8) . 2_545
O16 Mo5 Mo6 K2 -33.3(9) . 2_545
O23 Mo5 Mo6 K2 -175.9(7) . 2_545
O20 Mo5 Mo6 K2 -27.5(11) . 2_545
O14 Mo5 Mo6 K2 -178.4(9) . 2_545
O14 Mo5 Mo6 K2 -109.2(5) 2_655 2_545
Sr1 Mo5 Mo6 K2 -3.72(17) 1_655 2_545
O22 Mo5 Mo6 Sr1 -5.3(8) . 2_545
O16 Mo5 Mo6 Sr1 -115.2(9) . 2_545
O23 Mo5 Mo6 Sr1 102.1(7) . 2_545
O20 Mo5 Mo6 Sr1 -109.5(11) . 2_545
O14 Mo5 Mo6 Sr1 99.7(9) . 2_545
O14 Mo5 Mo6 Sr1 168.8(5) 2_655 2_545
Sr1 Mo5 Mo6 Sr1 -85.66(13) 1_655 2_545
O10 Th2 Mo6 O17 -123.3(11) 2 .
O16 Th2 Mo6 O17 -48.1(11) 1_455 .
O19 Th2 Mo6 O17 151.9(12) . .
O23 Th2 Mo6 O17 174.0(12) 2_655 .
O7 Th2 Mo6 O17 20.2(13) . .
O21 Th2 Mo6 O17 89.2(11) . .
O6 Th2 Mo6 O17 21.3(11) . .
O4 Th2 Mo6 O17 -31(2) . .
Mo2 Th2 Mo6 O17 24.1(10) . .
K2 Th2 Mo6 O17 -162.0(10) 2 .
Sr1 Th2 Mo6 O17 -13.6(10) . .
O10 Th2 Mo6 O10 -27.9(10) 2 .
O16 Th2 Mo6 O10 47.4(8) 1_455 .
O19 Th2 Mo6 O10 -112.6(8) . .
O23 Th2 Mo6 O10 -90.5(9) 2_655 .
O7 Th2 Mo6 O10 115.6(11) . .
O21 Th2 Mo6 O10 -175.3(8) . .
O6 Th2 Mo6 O10 116.8(8) . .
O4 Th2 Mo6 O10 64(2) . .
Mo2 Th2 Mo6 O10 119.6(6) . .
K2 Th2 Mo6 O10 -66.6(6) 2 .
Sr1 Th2 Mo6 O10 81.9(6) . .
O10 Th2 Mo6 O7 -143.5(10) 2 .
O16 Th2 Mo6 O7 -68.3(10) 1_455 .
O19 Th2 Mo6 O7 131.7(11) . .
O23 Th2 Mo6 O7 153.8(11) 2_655 .
O21 Th2 Mo6 O7 69.1(10) . .
O6 Th2 Mo6 O7 1.1(10) . .
O4 Th2 Mo6 O7 -51(2) . .
Mo2 Th2 Mo6 O7 4.0(9) . .
K2 Th2 Mo6 O7 177.8(9) 2 .
Sr1 Th2 Mo6 O7 -33.7(9) . .
O10 Th2 Mo6 O20 128.9(8) 2 .
O16 Th2 Mo6 O20 -155.8(9) 1_455 .
O19 Th2 Mo6 O20 44.2(9) . .
O23 Th2 Mo6 O20 66.3(10) 2_655 .
O7 Th2 Mo6 O20 -87.5(11) . .
O21 Th2 Mo6 O20 -18.5(8) . .
O6 Th2 Mo6 O20 -86.4(8) . .
O4 Th2 Mo6 O20 -139(2) . .
Mo2 Th2 Mo6 O20 -83.6(7) . .
K2 Th2 Mo6 O20 90.2(7) 2 .
Sr1 Th2 Mo6 O20 -121.3(7) . .
O10 Th2 Mo6 O14 56.0(8) 2 .
O16 Th2 Mo6 O14 131.2(9) 1_455 .
O19 Th2 Mo6 O14 -28.8(9) . .
O23 Th2 Mo6 O14 -6.7(9) 2_655 .
O7 Th2 Mo6 O14 -160.5(11) . .
O21 Th2 Mo6 O14 -91.5(8) . .
O6 Th2 Mo6 O14 -159.4(8) . .
O4 Th2 Mo6 O14 148(2) . .
Mo2 Th2 Mo6 O14 -156.5(7) . .
K2 Th2 Mo6 O14 17.3(7) 2 .
Sr1 Th2 Mo6 O14 165.7(7) . .
O10 Th2 Mo6 O23 62.7(8) 2 2_655
O16 Th2 Mo6 O23 137.9(9) 1_455 2_655
O19 Th2 Mo6 O23 -22.1(9) . 2_655
O7 Th2 Mo6 O23 -153.8(11) . 2_655
O21 Th2 Mo6 O23 -84.8(8) . 2_655
O6 Th2 Mo6 O23 -152.7(8) . 2_655
O4 Th2 Mo6 O23 155(2) . 2_655
Mo2 Th2 Mo6 O23 -149.9(7) . 2_655
K2 Th2 Mo6 O23 24.0(7) 2 2_655
Sr1 Th2 Mo6 O23 172.4(7) . 2_655
O10 Th2 Mo6 Mo5 99.8(5) 2 .
O16 Th2 Mo6 Mo5 175.0(6) 1_455 .
O19 Th2 Mo6 Mo5 15.0(6) . .
O23 Th2 Mo6 Mo5 37.1(7) 2_655 .
O7 Th2 Mo6 Mo5 -116.7(9) . .
O21 Th2 Mo6 Mo5 -47.7(4) . .
O6 Th2 Mo6 Mo5 -115.6(5) . .
O4 Th2 Mo6 Mo5 -168(2) . .
Mo2 Th2 Mo6 Mo5 -112.77(7) . .
K2 Th2 Mo6 Mo5 61.04(13) 2 .
Sr1 Th2 Mo6 Mo5 -150.47(9) . .
O10 Th2 Mo6 K2 -74.5(5) 2 .
O16 Th2 Mo6 K2 0.7(6) 1_455 .
O19 Th2 Mo6 K2 -159.3(6) . .
O23 Th2 Mo6 K2 -137.2(7) 2_655 .
O7 Th2 Mo6 K2 69.0(9) . .
O21 Th2 Mo6 K2 138.0(5) . .
O6 Th2 Mo6 K2 70.1(5) . .
O4 Th2 Mo6 K2 18(2) . .
Mo2 Th2 Mo6 K2 72.94(15) . .
K2 Th2 Mo6 K2 -113.25(15) 2 .
Sr1 Th2 Mo6 K2 35.23(16) . .
O10 Th2 Mo6 K2 -154.6(5) 2 2_545
O16 Th2 Mo6 K2 -79.4(6) 1_455 2_545
O19 Th2 Mo6 K2 120.6(6) . 2_545
O23 Th2 Mo6 K2 142.7(7) 2_655 2_545
O7 Th2 Mo6 K2 -11.1(9) . 2_545
O21 Th2 Mo6 K2 57.9(5) . 2_545
O6 Th2 Mo6 K2 -10.0(5) . 2_545
O4 Th2 Mo6 K2 -62(2) . 2_545
Mo2 Th2 Mo6 K2 -7.15(13) . 2_545
K2 Th2 Mo6 K2 166.7(2) 2 2_545
Sr1 Th2 Mo6 K2 -44.85(15) . 2_545
O10 Th2 Mo6 Sr1 -140.1(5) 2 2_545
O16 Th2 Mo6 Sr1 -64.9(6) 1_455 2_545
O19 Th2 Mo6 Sr1 135.1(6) . 2_545
O23 Th2 Mo6 Sr1 157.2(8) 2_655 2_545
O7 Th2 Mo6 Sr1 3.4(9) . 2_545
O21 Th2 Mo6 Sr1 72.4(5) . 2_545
O6 Th2 Mo6 Sr1 4.5(5) . 2_545
O4 Th2 Mo6 Sr1 -48(2) . 2_545
Mo2 Th2 Mo6 Sr1 7.3(3) . 2_545
K2 Th2 Mo6 Sr1 -178.9(3) 2 2_545
Sr1 Th2 Mo6 Sr1 -30.4(4) . 2_545
O18 Mo3 O1 Mo4 82.9(10) . 1_455
O24 Mo3 O1 Mo4 -171.4(10) . 1_455
O4 Mo3 O1 Mo4 -53(2) . 1_455
O2 Mo3 O1 Mo4 -14.1(9) 1_455 1_455
O12 Mo3 O1 Mo4 -89.2(9) . 1_455
K1 Mo3 O1 Mo4 142.5(8) 1_565 1_455
K1 Mo3 O1 Mo4 -120.3(10) 2_556 1_455
O18 Mo3 O1 Th1 -56(2) . 2_566
O24 Mo3 O1 Th1 50(2) . 2_566
O4 Mo3 O1 Th1 167.7(15) . 2_566
O2 Mo3 O1 Th1 -153(2) 1_455 2_566
O12 Mo3 O1 Th1 132(2) . 2_566
Mo4 Mo3 O1 Th1 -139(3) 1_455 2_566
K1 Mo3 O1 Th1 3.6(19) 1_565 2_566
K1 Mo3 O1 Th1 101(2) 2_556 2_566
O18 Mo3 O1 K1 -156.8(8) . 2_556
O24 Mo3 O1 K1 -51.1(9) . 2_556
O4 Mo3 O1 K1 67(2) . 2_556
O2 Mo3 O1 K1 106.2(8) 1_455 2_556
O12 Mo3 O1 K1 31.2(6) . 2_556
Mo4 Mo3 O1 K1 120.3(10) 1_455 2_556
K1 Mo3 O1 K1 -97.2(5) 1_565 2_556
O11 Mo4 O2 Mo3 76.1(11) . 1_655
O19 Mo4 O2 Mo3 177.9(10) . 1_655
O8 Mo4 O2 Mo3 -58.8(19) . 1_655
O1 Mo4 O2 Mo3 -14.1(9) 1_655 1_655
O13 Mo4 O2 Mo3 -95.1(9) . 1_655
Th1 Mo4 O2 Mo3 -10.2(11) 2_666 1_655
Th1 Mo4 O2 Mo3 -95.2(8) . 1_655
K2 Mo4 O2 Mo3 127.7(6) 2 1_655
O11 Mo4 O2 Mo1 -175.3(8) . .
O19 Mo4 O2 Mo1 -73.5(9) . .
O8 Mo4 O2 Mo1 49.8(18) . .
O1 Mo4 O2 Mo1 94.5(9) 1_655 .
O13 Mo4 O2 Mo1 13.5(6) . .
Mo3 Mo4 O2 Mo1 108.6(11) 1_655 .
Th1 Mo4 O2 Mo1 98.4(6) 2_666 .
Th1 Mo4 O2 Mo1 13.4(9) . .
K2 Mo4 O2 Mo1 -123.7(5) 2 .
O21 Mo1 O2 Mo4 81.0(9) . .
O5 Mo1 O2 Mo4 -84(4) . .
O3 Mo1 O2 Mo4 174.8(9) . .
O13 Mo1 O2 Mo4 -15.8(8) . .
O12 Mo1 O2 Mo4 -107.2(9) 1_655 .
Mo2 Mo1 O2 Mo4 -145.4(7) 1_655 .
K1 Mo1 O2 Mo4 -69.2(7) 2_656 .
K1 Mo1 O2 Mo4 40.0(15) . .
O21 Mo1 O2 Mo3 -171.4(10) . 1_655
O5 Mo1 O2 Mo3 24(5) . 1_655
O3 Mo1 O2 Mo3 -77.6(9) . 1_655
O13 Mo1 O2 Mo3 91.8(9) . 1_655
O12 Mo1 O2 Mo3 0.4(8) 1_655 1_655
Mo2 Mo1 O2 Mo3 -37.9(7) 1_655 1_655
K1 Mo1 O2 Mo3 38.3(7) 2_656 1_655
K1 Mo1 O2 Mo3 147.6(6) . 1_655
O21 Mo1 O3 Mo2 177.2(9) . 1_655
O5 Mo1 O3 Mo2 -75.3(10) . 1_655
O13 Mo1 O3 Mo2 71.3(19) . 1_655
O12 Mo1 O3 Mo2 20.2(8) 1_655 1_655
O2 Mo1 O3 Mo2 93.3(9) . 1_655
K1 Mo1 O3 Mo2 9.0(10) 2_656 1_655
K1 Mo1 O3 Mo2 -109.0(7) . 1_655
O21 Mo1 O3 Sr1 -51.6(18) . 1_655
O5 Mo1 O3 Sr1 55.9(18) . 1_655
O13 Mo1 O3 Sr1 -157.5(13) . 1_655
O12 Mo1 O3 Sr1 151.4(18) 1_655 1_655
O2 Mo1 O3 Sr1 -135.5(17) . 1_655
Mo2 Mo1 O3 Sr1 131(2) 1_655 1_655
K1 Mo1 O3 Sr1 140.2(14) 2_656 1_655
K1 Mo1 O3 Sr1 22.1(19) . 1_655
O18 Mo3 O4 Mo2 173.1(9) . .
O24 Mo3 O4 Mo2 67.8(11) . .
O1 Mo3 O4 Mo2 -50(2) . .
O2 Mo3 O4 Mo2 -87.5(9) 1_455 .
O12 Mo3 O4 Mo2 -12.6(7) . .
Mo4 Mo3 O4 Mo2 -87.2(8) 1_455 .
K1 Mo3 O4 Mo2 111.5(7) 1_565 .
K1 Mo3 O4 Mo2 4.2(9) 2_556 .
O18 Mo3 O4 Th2 23.3(19) . .
O24 Mo3 O4 Th2 -81.9(19) . .
O1 Mo3 O4 Th2 160.4(16) . .
O2 Mo3 O4 Th2 122.8(18) 1_455 .
O12 Mo3 O4 Th2 -162.3(19) . .
Mo4 Mo3 O4 Th2 123.1(15) 1_455 .
K1 Mo3 O4 Th2 -38(2) 1_565 .
K1 Mo3 O4 Th2 -145.5(15) 2_556 .
O15 Mo2 O4 Mo3 72(4) . .
O6 Mo2 O4 Mo3 -178.8(10) . .
O9 Mo2 O4 Mo3 -76.9(10) . .
O12 Mo2 O4 Mo3 14.0(8) . .
O3 Mo2 O4 Mo3 91.2(10) 1_455 .
Mo1 Mo2 O4 Mo3 55.9(7) 1_455 .
K1 Mo2 O4 Mo3 -122.9(7) . .
Th2 Mo2 O4 Mo3 -164.4(12) . .
Sr1 Mo2 O4 Mo3 134.6(7) . .
O15 Mo2 O4 Th2 -123(4) . .
O6 Mo2 O4 Th2 -14.3(8) . .
O9 Mo2 O4 Th2 87.6(8) . .
O12 Mo2 O4 Th2 178.4(8) . .
O3 Mo2 O4 Th2 -104.3(8) 1_455 .
Mo1 Mo2 O4 Th2 -139.7(5) 1_455 .
K1 Mo2 O4 Th2 41.5(10) . .
Sr1 Mo2 O4 Th2 -60.9(5) . .
O10 Th2 O4 Mo3 -47.8(18) 2 .
O16 Th2 O4 Mo3 -124.0(19) 1_455 .
O19 Th2 O4 Mo3 36.2(17) . .
O23 Th2 O4 Mo3 6(3) 2_655 .
O7 Th2 O4 Mo3 -179.4(14) . .
O21 Th2 O4 Mo3 100.5(18) . .
O6 Th2 O4 Mo3 162(2) . .
Mo6 Th2 O4 Mo3 -141.1(13) . .
Mo2 Th2 O4 Mo3 151(2) . .
K2 Th2 O4 Mo3 -7.4(16) 2 .
Sr1 Th2 O4 Mo3 -159.3(19) . .
O10 Th2 O4 Mo2 161.1(7) 2 .
O16 Th2 O4 Mo2 84.9(8) 1_455 .
O19 Th2 O4 Mo2 -114.9(8) . .
O23 Th2 O4 Mo2 -145.4(10) 2_655 .
O7 Th2 O4 Mo2 29.6(13) . .
O21 Th2 O4 Mo2 -50.6(8) . .
O6 Th2 O4 Mo2 11.3(6) . .
Mo6 Th2 O4 Mo2 68(2) . .
K2 Th2 O4 Mo2 -158.4(7) 2 .
Sr1 Th2 O4 Mo2 49.7(5) . .
O21 Mo1 O5 Th1 136.1(15) . 2_656
O3 Mo1 O5 Th1 39.6(17) . 2_656
O13 Mo1 O5 Th1 -125.0(15) . 2_656
O12 Mo1 O5 Th1 -37.4(16) 1_655 2_656
O2 Mo1 O5 Th1 -60(5) . 2_656
Mo2 Mo1 O5 Th1 1.5(15) 1_655 2_656
K1 Mo1 O5 Th1 -74.4(14) 2_656 2_656
K1 Mo1 O5 Th1 163(2) . 2_656
O21 Mo1 O5 K1 -26.5(13) . .
O3 Mo1 O5 K1 -123.0(10) . .
O13 Mo1 O5 K1 72.4(11) . .
O12 Mo1 O5 K1 160.0(10) 1_655 .
O2 Mo1 O5 K1 137(4) . .
Mo2 Mo1 O5 K1 -161.1(9) 1_655 .
K1 Mo1 O5 K1 123.0(10) 2_656 .
O15 Mo2 O6 Th2 -176.6(9) . .
O9 Mo2 O6 Th2 -70.8(10) . .
O12 Mo2 O6 Th2 44(2) . .
O3 Mo2 O6 Th2 93.1(9) 1_455 .
O4 Mo2 O6 Th2 15.2(8) . .
Mo1 Mo2 O6 Th2 94.0(8) 1_455 .
K1 Mo2 O6 Th2 -129.2(8) . .
Sr1 Mo2 O6 Th2 117.4(11) . .
O15 Mo2 O6 Sr1 66.0(9) . .
O9 Mo2 O6 Sr1 171.7(8) . .
O12 Mo2 O6 Sr1 -73(2) . .
O3 Mo2 O6 Sr1 -24.4(8) 1_455 .
O4 Mo2 O6 Sr1 -102.2(8) . .
Mo1 Mo2 O6 Sr1 -23.4(10) 1_455 .
K1 Mo2 O6 Sr1 113.4(7) . .
Th2 Mo2 O6 Sr1 -117.4(11) . .
O15 Mo2 O6 K1 -47.4(7) . .
O9 Mo2 O6 K1 58.3(7) . .
O12 Mo2 O6 K1 173.2(16) . .
O3 Mo2 O6 K1 -137.8(6) 1_455 .
O4 Mo2 O6 K1 144.4(6) . .
Mo1 Mo2 O6 K1 -136.8(4) 1_455 .
Th2 Mo2 O6 K1 129.2(8) . .
Sr1 Mo2 O6 K1 -113.4(7) . .
O10 Th2 O6 Mo2 -61.7(13) 2 .
O16 Th2 O6 Mo2 -105.9(11) 1_455 .
O19 Th2 O6 Mo2 40.3(11) . .
O23 Th2 O6 Mo2 146.3(9) 2_655 .
O7 Th2 O6 Mo2 176.5(10) . .
O21 Th2 O6 Mo2 101.4(10) . .
O4 Th2 O6 Mo2 -14.5(8) . .
Mo6 Th2 O6 Mo2 175.9(7) . .
K2 Th2 O6 Mo2 0.6(13) 2 .
Sr1 Th2 O6 Mo2 -113.9(12) . .
O10 Th2 O6 Sr1 52.1(12) 2 .
O16 Th2 O6 Sr1 7.9(8) 1_455 .
O19 Th2 O6 Sr1 154.1(7) . .
O23 Th2 O6 Sr1 -99.8(11) 2_655 .
O7 Th2 O6 Sr1 -69.7(7) . .
O21 Th2 O6 Sr1 -144.8(9) . .
O4 Th2 O6 Sr1 99.4(8) . .
Mo6 Th2 O6 Sr1 -70.2(7) . .
Mo2 Th2 O6 Sr1 113.9(12) . .
K2 Th2 O6 Sr1 114.5(6) 2 .
O10 Th2 O6 K1 -151.7(8) 2 .
O16 Th2 O6 K1 164.1(11) 1_455 .
O19 Th2 O6 K1 -49.7(11) . .
O23 Th2 O6 K1 56.3(14) 2_655 .
O7 Th2 O6 K1 86.5(10) . .
O21 Th2 O6 K1 11.4(9) . .
O4 Th2 O6 K1 -104.5(10) . .
Mo6 Th2 O6 K1 85.9(9) . .
Mo2 Th2 O6 K1 -90.0(12) . .
K2 Th2 O6 K1 -89.4(10) 2 .
Sr1 Th2 O6 K1 156.1(14) . .
O17 Mo6 O7 Th2 -166.5(9) . .
O10 Mo6 O7 Th2 -66.0(9) . .
O20 Mo6 O7 Th2 95.8(9) . .
O14 Mo6 O7 Th2 41(2) . .
O23 Mo6 O7 Th2 17.7(8) 2_655 .
Mo5 Mo6 O7 Th2 92.2(8) . .
K2 Mo6 O7 Th2 -117.7(7) . .
K2 Mo6 O7 Th2 160.5(15) 2_545 .
Sr1 Mo6 O7 Th2 -178.8(3) 2_545 .
O17 Mo6 O7 K2 33.0(12) . 2_545
O10 Mo6 O7 K2 133.5(10) . 2_545
O20 Mo6 O7 K2 -64.7(11) . 2_545
O14 Mo6 O7 K2 -119.8(17) . 2_545
O23 Mo6 O7 K2 -142.8(10) 2_655 2_545
Mo5 Mo6 O7 K2 -68.3(11) . 2_545
Th2 Mo6 O7 K2 -160.5(15) . 2_545
K2 Mo6 O7 K2 81.8(9) . 2_545
Sr1 Mo6 O7 K2 20.7(12) 2_545 2_545
O10 Th2 O7 Mo6 41.9(11) 2 .
O16 Th2 O7 Mo6 107.2(10) 1_455 .
O19 Th2 O7 Mo6 -67.7(13) . .
O23 Th2 O7 Mo6 -18.1(8) 2_655 .
O21 Th2 O7 Mo6 -105.0(9) . .
O6 Th2 O7 Mo6 -178.9(9) . .
O4 Th2 O7 Mo6 164.6(8) . .
Mo2 Th2 O7 Mo6 -177.2(6) . .
K2 Th2 O7 Mo6 -3.2(13) 2 .
Sr1 Th2 O7 Mo6 144.2(9) . .
O10 Th2 O7 K2 -157.0(8) 2 2_545
O16 Th2 O7 K2 -91.8(10) 1_455 2_545
O19 Th2 O7 K2 93.4(11) . 2_545
O23 Th2 O7 K2 143.0(10) 2_655 2_545
O21 Th2 O7 K2 56.1(8) . 2_545
O6 Th2 O7 K2 -17.8(8) . 2_545
O4 Th2 O7 K2 -34.3(14) . 2_545
Mo6 Th2 O7 K2 161.1(15) . 2_545
Mo2 Th2 O7 K2 -16.1(9) . 2_545
K2 Th2 O7 K2 157.9(5) 2 2_545
Sr1 Th2 O7 K2 -54.7(7) . 2_545
O11 Mo4 O8 Th1 169.4(9) . .
O19 Mo4 O8 Th1 67.7(10) . .
O2 Mo4 O8 Th1 -54.5(19) . .
O1 Mo4 O8 Th1 -97.5(9) 1_655 .
O13 Mo4 O8 Th1 -18.3(7) . .
Mo3 Mo4 O8 Th1 -93.1(7) 1_655 .
Th1 Mo4 O8 Th1 -123.1(11) 2_666 .
K2 Mo4 O8 Th1 119.7(7) 2 .
O11 Mo4 O8 Th1 -67.5(9) . 2_666
O19 Mo4 O8 Th1 -169.2(8) . 2_666
O2 Mo4 O8 Th1 68.6(18) . 2_666
O1 Mo4 O8 Th1 25.6(8) 1_655 2_666
O13 Mo4 O8 Th1 104.8(8) . 2_666
Mo3 Mo4 O8 Th1 30.0(9) 1_655 2_666
Th1 Mo4 O8 Th1 123.1(11) . 2_666
K2 Mo4 O8 Th1 -117.1(6) 2 2_666
O11 Mo4 O8 K1 44.0(13) . 1_565
O19 Mo4 O8 K1 -57.7(14) . 1_565
O2 Mo4 O8 K1 -179.9(12) . 1_565
O1 Mo4 O8 K1 137.1(12) 1_655 1_565
O13 Mo4 O8 K1 -143.7(13) . 1_565
Mo3 Mo4 O8 K1 141.5(9) 1_655 1_565
Th1 Mo4 O8 K1 111.5(14) 2_666 1_565
Th1 Mo4 O8 K1 -125.4(15) . 1_565
K2 Mo4 O8 K1 -5.7(11) 2 1_565
O24 Th1 O8 Mo4 -102.5(10) . .
O13 Th1 O8 Mo4 18.8(7) . .
O9 Th1 O8 Mo4 -41.3(11) . .
O15 Th1 O8 Mo4 -147.2(13) 2_556 .
O1 Th1 O8 Mo4 179.9(10) 2_566 .
O5 Th1 O8 Mo4 66.6(11) 2_656 .
O8 Th1 O8 Mo4 114.6(13) 2_666 .
Mo4 Th1 O8 Mo4 142.7(8) 2_666 .
K1 Th1 O8 Mo4 73.4(8) 2_656 .
K1 Th1 O8 Mo4 -141.7(12) 1_565 .
O24 Th1 O8 Th1 142.9(10) . 2_666
O13 Th1 O8 Th1 -95.8(9) . 2_666
O9 Th1 O8 Th1 -155.9(7) . 2_666
O15 Th1 O8 Th1 98.2(16) 2_556 2_666
O1 Th1 O8 Th1 65.4(8) 2_566 2_666
O5 Th1 O8 Th1 -48.0(11) 2_656 2_666
O8 Th1 O8 Th1 0.0 2_666 2_666
Mo4 Th1 O8 Th1 28.2(7) 2_666 2_666
Mo4 Th1 O8 Th1 -114.6(13) . 2_666
K1 Th1 O8 Th1 -41.2(7) 2_656 2_666
K1 Th1 O8 Th1 103.8(10) 1_565 2_666
O24 Th1 O8 K1 39.1(7) . 1_565
O13 Th1 O8 K1 160.4(8) . 1_565
O9 Th1 O8 K1 100.4(7) . 1_565
O15 Th1 O8 K1 -5.6(19) 2_556 1_565
O1 Th1 O8 K1 -38.4(7) 2_566 1_565
O5 Th1 O8 K1 -151.8(6) 2_656 1_565
O8 Th1 O8 K1 -103.8(10) 2_666 1_565
Mo4 Th1 O8 K1 -75.6(5) 2_666 1_565
Mo4 Th1 O8 K1 141.7(12) . 1_565
K1 Th1 O8 K1 -145.0(5) 2_656 1_565
O15 Mo2 O9 Th1 -122(2) . .
O6 Mo2 O9 Th1 134(2) . .
O12 Mo2 O9 Th1 -22(2) . .
O3 Mo2 O9 Th1 13(4) 1_455 .
O4 Mo2 O9 Th1 52(2) . .
Mo1 Mo2 O9 Th1 -29(3) 1_455 .
K1 Mo2 O9 Th1 -161(2) . .
Th2 Mo2 O9 Th1 96(2) . .
Sr1 Mo2 O9 Th1 146.1(14) . .
O15 Mo2 O9 K1 39.0(8) . .
O6 Mo2 O9 K1 -64.7(8) . .
O12 Mo2 O9 K1 138.9(7) . .
O3 Mo2 O9 K1 174(2) 1_455 .
O4 Mo2 O9 K1 -147.5(6) . .
Mo1 Mo2 O9 K1 132.3(5) 1_455 .
Th2 Mo2 O9 K1 -103.2(4) . .
Sr1 Mo2 O9 K1 -52.9(13) . .
O24 Th1 O9 Mo2 -14(2) . .
O13 Th1 O9 Mo2 -130(2) . .
O15 Th1 O9 Mo2 80(2) 2_556 .
O1 Th1 O9 Mo2 30(3) 2_566 .
O8 Th1 O9 Mo2 -76(2) . .
O5 Th1 O9 Mo2 153(2) 2_656 .
O8 Th1 O9 Mo2 -156.5(17) 2_666 .
Mo4 Th1 O9 Mo2 90(3) 2_666 .
Mo4 Th1 O9 Mo2 -95(2) . .
K1 Th1 O9 Mo2 -168(2) 2_656 .
K1 Th1 O9 Mo2 -30(2) 1_565 .
O24 Th1 O9 K1 -171.1(11) . .
O13 Th1 O9 K1 72.4(9) . .
O15 Th1 O9 K1 -77.7(9) 2_556 .
O1 Th1 O9 K1 -127.7(10) 2_566 .
O8 Th1 O9 K1 126.6(8) . .
O5 Th1 O9 K1 -4.0(9) 2_656 .
O8 Th1 O9 K1 46(2) 2_666 .
Mo4 Th1 O9 K1 -68(2) 2_666 .
Mo4 Th1 O9 K1 107.3(8) . .
K1 Th1 O9 K1 34.7(10) 2_656 .
K1 Th1 O9 K1 172.3(6) 1_565 .
O17 Mo6 O10 Th2 -132(2) . 2
O7 Mo6 O10 Th2 126(2) . 2
O20 Mo6 O10 Th2 -2(4) . 2
O14 Mo6 O10 Th2 -29(2) . 2
O23 Mo6 O10 Th2 47(2) 2_655 2
Mo5 Mo6 O10 Th2 -34(2) . 2
Th2 Mo6 O10 Th2 90(2) . 2
K2 Mo6 O10 Th2 -151(3) . 2
K2 Mo6 O10 Th2 153.7(18) 2_545 2
Sr1 Mo6 O10 Th2 -107(2) 2_545 2
O17 Mo6 O10 K2 18.8(9) . .
O7 Mo6 O10 K2 -83.4(8) . .
O20 Mo6 O10 K2 149.4(19) . .
O14 Mo6 O10 K2 122.3(8) . .
O23 Mo6 O10 K2 -162.0(8) 2_655 .
Mo5 Mo6 O10 K2 116.9(5) . .
Th2 Mo6 O10 K2 -119.1(6) . .
K2 Mo6 O10 K2 -55.4(8) 2_545 .
Sr1 Mo6 O10 K2 43.8(6) 2_545 .
O19 Mo4 O11 Sr1 -108.9(15) . 1_665
O8 Mo4 O11 Sr1 148.1(15) . 1_665
O2 Mo4 O11 Sr1 -9.6(17) . 1_665
O1 Mo4 O11 Sr1 65.0(15) 1_655 1_665
O13 Mo4 O11 Sr1 87(6) . 1_665
Mo3 Mo4 O11 Sr1 29.0(14) 1_655 1_665
Th1 Mo4 O11 Sr1 106.0(14) 2_666 1_665
Th1 Mo4 O11 Sr1 158.5(8) . 1_665
K2 Mo4 O11 Sr1 -122.5(18) 2 1_665
O19 Mo4 O11 K2 13.6(10) . 2
O8 Mo4 O11 K2 -89.4(8) . 2
O2 Mo4 O11 K2 112.9(8) . 2
O1 Mo4 O11 K2 -172.5(8) 1_655 2
O13 Mo4 O11 K2 -150(5) . 2
Mo3 Mo4 O11 K2 151.5(6) 1_655 2
Th1 Mo4 O11 K2 -131.6(7) 2_666 2
Th1 Mo4 O11 K2 -79.0(10) . 2
O15 Mo2 O12 Mo1 -69.5(9) . 1_455
O6 Mo2 O12 Mo1 70(2) . 1_455
O9 Mo2 O12 Mo1 -172.8(9) . 1_455
O3 Mo2 O12 Mo1 18.4(8) 1_455 1_455
O4 Mo2 O12 Mo1 99.9(8) . 1_455
K1 Mo2 O12 Mo1 -118.9(6) . 1_455
Th2 Mo2 O12 Mo1 101.1(6) . 1_455
Sr1 Mo2 O12 Mo1 14.4(10) . 1_455
O15 Mo2 O12 Mo3 179.2(8) . .
O6 Mo2 O12 Mo3 -41(2) . .
O9 Mo2 O12 Mo3 75.9(9) . .
O3 Mo2 O12 Mo3 -92.9(9) 1_455 .
O4 Mo2 O12 Mo3 -11.4(7) . .
Mo1 Mo2 O12 Mo3 -111.3(10) 1_455 .
K1 Mo2 O12 Mo3 129.8(5) . .
Th2 Mo2 O12 Mo3 -10.2(8) . .
Sr1 Mo2 O12 Mo3 -96.9(6) . .
O15 Mo2 O12 K1 56.0(14) . 2_556
O6 Mo2 O12 K1 -164.5(15) . 2_556
O9 Mo2 O12 K1 -47.2(14) . 2_556
O3 Mo2 O12 K1 144.0(14) 1_455 2_556
O4 Mo2 O12 K1 -134.5(14) . 2_556
Mo1 Mo2 O12 K1 125.5(17) 1_455 2_556
K1 Mo2 O12 K1 6.7(17) . 2_556
Th2 Mo2 O12 K1 -133.3(11) . 2_556
Sr1 Mo2 O12 K1 139.9(10) . 2_556
O18 Mo3 O12 Mo2 45(5) . .
O24 Mo3 O12 Mo2 -86.4(10) . .
O4 Mo3 O12 Mo2 12.9(8) . .
O1 Mo3 O12 Mo2 177.7(9) . .
O2 Mo3 O12 Mo2 102.8(9) 1_455 .
Mo4 Mo3 O12 Mo2 137.8(6) 1_455 .
K1 Mo3 O12 Mo2 -104.9(6) 1_565 .
K1 Mo3 O12 Mo2 -143.8(11) 2_556 .
O18 Mo3 O12 Mo1 -57(5) . 1_455
O24 Mo3 O12 Mo1 171.2(11) . 1_455
O4 Mo3 O12 Mo1 -89.5(9) . 1_455
O1 Mo3 O12 Mo1 75.3(9) . 1_455
O2 Mo3 O12 Mo1 0.4(8) 1_455 1_455
Mo4 Mo3 O12 Mo1 35.4(7) 1_455 1_455
K1 Mo3 O12 Mo1 152.7(4) 1_565 1_455
K1 Mo3 O12 Mo1 113.8(11) 2_556 1_455
O18 Mo3 O12 K1 -171(5) . 2_556
O24 Mo3 O12 K1 57.4(9) . 2_556
O4 Mo3 O12 K1 156.8(9) . 2_556
O1 Mo3 O12 K1 -38.4(8) . 2_556
O2 Mo3 O12 K1 -113.3(9) 1_455 2_556
Mo4 Mo3 O12 K1 -78.4(6) 1_455 2_556
K1 Mo3 O12 K1 38.9(9) 1_565 2_556
O21 Mo1 O13 Mo4 -68.6(9) . .
O5 Mo1 O13 Mo4 -176.7(8) . .
O3 Mo1 O13 Mo4 37(2) . .
O12 Mo1 O13 Mo4 85.9(8) 1_655 .
O2 Mo1 O13 Mo4 14.1(7) . .
Mo2 Mo1 O13 Mo4 84.8(8) 1_655 .
K1 Mo1 O13 Mo4 114.8(9) 2_656 .
K1 Mo1 O13 Mo4 -142.9(6) . .
O21 Mo1 O13 Th1 80.0(17) . .
O5 Mo1 O13 Th1 -28.1(18) . .
O3 Mo1 O13 Th1 -174.7(14) . .
O12 Mo1 O13 Th1 -125.5(17) 1_655 .
O2 Mo1 O13 Th1 162.7(18) . .
Mo2 Mo1 O13 Th1 -126.6(14) 1_655 .
K1 Mo1 O13 Th1 -96.6(17) 2_656 .
K1 Mo1 O13 Th1 5.7(16) . .
O21 Mo1 O13 K1 176.6(7) . 2_656
O5 Mo1 O13 K1 68.5(8) . 2_656
O3 Mo1 O13 K1 -78.1(17) . 2_656
O12 Mo1 O13 K1 -29.0(7) 1_655 2_656
O2 Mo1 O13 K1 -100.8(7) . 2_656
Mo2 Mo1 O13 K1 -30.0(8) 1_655 2_656
K1 Mo1 O13 K1 102.2(4) . 2_656
O11 Mo4 O13 Mo1 -116(6) . .
O19 Mo4 O13 Mo1 80.0(10) . .
O8 Mo4 O13 Mo1 -178.2(9) . .
O2 Mo4 O13 Mo1 -16.9(8) . .
O1 Mo4 O13 Mo1 -93.2(9) 1_655 .
Mo3 Mo4 O13 Mo1 -57.0(6) 1_655 .
Th1 Mo4 O13 Mo1 -134.3(6) 2_666 .
Th1 Mo4 O13 Mo1 163.1(12) . .
K2 Mo4 O13 Mo1 98.3(8) 2 .
O11 Mo4 O13 Th1 81(6) . .
O19 Mo4 O13 Th1 -83.1(8) . .
O8 Mo4 O13 Th1 18.7(7) . .
O2 Mo4 O13 Th1 -180.0(9) . .
O1 Mo4 O13 Th1 103.7(8) 1_655 .
Mo3 Mo4 O13 Th1 139.9(6) 1_655 .
Th1 Mo4 O13 Th1 62.6(5) 2_666 .
K2 Mo4 O13 Th1 -64.8(9) 2 .
O11 Mo4 O13 K1 -13(6) . 2_656
O19 Mo4 O13 K1 -177.3(9) . 2_656
O8 Mo4 O13 K1 -75.5(8) . 2_656
O2 Mo4 O13 K1 85.8(8) . 2_656
O1 Mo4 O13 K1 9.5(7) 1_655 2_656
Mo3 Mo4 O13 K1 45.6(5) 1_655 2_656
Th1 Mo4 O13 K1 -31.7(6) 2_666 2_656
Th1 Mo4 O13 K1 -94.2(8) . 2_656
K2 Mo4 O13 K1 -159.0(3) 2 2_656
O24 Th1 O13 Mo1 -103.7(17) . .
O9 Th1 O13 Mo1 -39.0(16) . .
O15 Th1 O13 Mo1 7(2) 2_556 .
O1 Th1 O13 Mo1 163.8(13) 2_566 .
O8 Th1 O13 Mo1 -164.4(19) . .
O5 Th1 O13 Mo1 53.0(16) 2_656 .
O8 Th1 O13 Mo1 131.4(17) 2_666 .
Mo4 Th1 O13 Mo1 129.3(15) 2_666 .
Mo4 Th1 O13 Mo1 -149(2) . .
K1 Th1 O13 Mo1 98.4(17) 2_656 .
K1 Th1 O13 Mo1 -151.1(15) 1_565 .
O24 Th1 O13 Mo4 45.4(9) . .
O9 Th1 O13 Mo4 110.1(8) . .
O15 Th1 O13 Mo4 156.1(8) 2_556 .
O1 Th1 O13 Mo4 -47.2(13) 2_566 .
O8 Th1 O13 Mo4 -15.3(6) . .
O5 Th1 O13 Mo4 -157.9(8) 2_656 .
O8 Th1 O13 Mo4 -79.5(7) 2_666 .
Mo4 Th1 O13 Mo4 -81.7(6) 2_666 .
K1 Th1 O13 Mo4 -112.5(7) 2_656 .
K1 Th1 O13 Mo4 -2.1(7) 1_565 .
O24 Th1 O13 K1 157.9(6) . 2_656
O9 Th1 O13 K1 -137.4(6) . 2_656
O15 Th1 O13 K1 -91.4(9) 2_556 2_656
O1 Th1 O13 K1 65.3(11) 2_566 2_656
O8 Th1 O13 K1 97.2(6) . 2_656
O5 Th1 O13 K1 -45.4(5) 2_656 2_656
O8 Th1 O13 K1 33.0(6) 2_666 2_656
Mo4 Th1 O13 K1 30.9(6) 2_666 2_656
Mo4 Th1 O13 K1 112.5(7) . 2_656
K1 Th1 O13 K1 110.4(3) 1_565 2_656
O22 Mo5 O14 Mo6 79.9(11) . .
O16 Mo5 O14 Mo6 -69(2) . .
O23 Mo5 O14 Mo6 -178.1(9) . .
O20 Mo5 O14 Mo6 -18.0(8) . .
O14 Mo5 O14 Mo6 -102.5(11) 2_655 .
Sr1 Mo5 O14 Mo6 -6.2(11) 1_655 .
O22 Mo5 O14 Mo5 -177.6(10) . 2_655
O16 Mo5 O14 Mo5 34(2) . 2_655
O23 Mo5 O14 Mo5 -75.6(9) . 2_655
O20 Mo5 O14 Mo5 84.5(10) . 2_655
O14 Mo5 O14 Mo5 -0.002(1) 2_655 2_655
Mo6 Mo5 O14 Mo5 102.5(11) . 2_655
Sr1 Mo5 O14 Mo5 96.3(8) 1_655 2_655
O17 Mo6 O14 Mo5 -75.1(10) . .
O10 Mo6 O14 Mo5 -172.9(9) . .
O7 Mo6 O14 Mo5 77(2) . .
O20 Mo6 O14 Mo5 17.9(8) . .
O23 Mo6 O14 Mo5 100.7(9) 2_655 .
Th2 Mo6 O14 Mo5 105.4(7) . .
K2 Mo6 O14 Mo5 -126.3(6) . .
K2 Mo6 O14 Mo5 3.0(17) 2_545 .
Sr1 Mo6 O14 Mo5 -69.6(7) 2_545 .
O17 Mo6 O14 Mo5 174.7(8) . 2_655
O10 Mo6 O14 Mo5 76.9(8) . 2_655
O7 Mo6 O14 Mo5 -33(2) . 2_655
O20 Mo6 O14 Mo5 -92.2(9) . 2_655
O23 Mo6 O14 Mo5 -9.5(7) 2_655 2_655
Mo5 Mo6 O14 Mo5 -110.2(10) . 2_655
Th2 Mo6 O14 Mo5 -4.8(9) . 2_655
K2 Mo6 O14 Mo5 123.5(5) . 2_655
K2 Mo6 O14 Mo5 -107.2(10) 2_545 2_655
Sr1 Mo6 O14 Mo5 -179.7(7) 2_545 2_655
O6 Mo2 O15 Th1 -151.2(19) . 2_556
O9 Mo2 O15 Th1 104.2(19) . 2_556
O12 Mo2 O15 Th1 12(2) . 2_556
O3 Mo2 O15 Th1 -62.6(19) 1_455 2_556
O4 Mo2 O15 Th1 -44(5) . 2_556
Mo1 Mo2 O15 Th1 -27.6(18) 1_455 2_556
K1 Mo2 O15 Th1 149(2) . 2_556
Th2 Mo2 O15 Th1 -154.9(12) . 2_556
Sr1 Mo2 O15 Th1 -107.8(19) . 2_556
O6 Mo2 O15 K1 60.3(8) . .
O9 Mo2 O15 K1 -44.3(9) . .
O12 Mo2 O15 K1 -136.7(7) . .
O3 Mo2 O15 K1 148.9(8) 1_455 .
O4 Mo2 O15 K1 167(3) . .
Mo1 Mo2 O15 K1 -176.1(5) 1_455 .
Th2 Mo2 O15 K1 56.6(11) . .
Sr1 Mo2 O15 K1 103.7(5) . .
O22 Mo5 O16 Th2 117(2) . 1_655
O23 Mo5 O16 Th2 12(2) . 1_655
O20 Mo5 O16 Th2 -143(2) . 1_655
O14 Mo5 O16 Th2 -94(3) . 1_655
O14 Mo5 O16 Th2 -62(2) 2_655 1_655
Mo6 Mo5 O16 Th2 -139.7(17) . 1_655
Sr1 Mo5 O16 Th2 -180(3) 1_655 1_655
O22 Mo5 O16 Sr1 -62.7(11) . 1_655
O23 Mo5 O16 Sr1 -168.3(8) . 1_655
O20 Mo5 O16 Sr1 36.7(9) . 1_655
O14 Mo5 O16 Sr1 85.5(19) . 1_655
O14 Mo5 O16 Sr1 117.7(9) 2_655 1_655
Mo6 Mo5 O16 Sr1 40.3(10) . 1_655
O10 Mo6 O17 Sr1 102.3(16) . 2_545
O7 Mo6 O17 Sr1 -154.8(15) . 2_545
O20 Mo6 O17 Sr1 -60.2(17) . 2_545
O14 Mo6 O17 Sr1 13.0(17) . 2_545
O23 Mo6 O17 Sr1 -67(13) 2_655 2_545
Mo5 Mo6 O17 Sr1 -23.5(15) . 2_545
Th2 Mo6 O17 Sr1 -167.6(8) . 2_545
K2 Mo6 O17 Sr1 122.0(19) . 2_545
K2 Mo6 O17 Sr1 -136.5(16) 2_545 2_545
O10 Mo6 O17 K2 -19.6(10) . .
O7 Mo6 O17 K2 83.2(9) . .
O20 Mo6 O17 K2 177.8(8) . .
O14 Mo6 O17 K2 -109.0(8) . .
O23 Mo6 O17 K2 171(12) 2_655 .
Mo5 Mo6 O17 K2 -145.5(6) . .
Th2 Mo6 O17 K2 70.4(11) . .
K2 Mo6 O17 K2 101.5(7) 2_545 .
Sr1 Mo6 O17 K2 -122.0(19) 2_545 .
O24 Mo3 O18 Sr1 -143.2(13) . 1_565
O4 Mo3 O18 Sr1 117.9(13) . 1_565
O1 Mo3 O18 Sr1 -44.6(14) . 1_565
O2 Mo3 O18 Sr1 31.1(14) 1_455 1_565
O12 Mo3 O18 Sr1 86(5) . 1_565
Mo4 Mo3 O18 Sr1 -5.0(12) 1_455 1_565
K1 Mo3 O18 Sr1 -120.0(14) 1_565 1_565
K1 Mo3 O18 Sr1 -81.6(17) 2_556 1_565
O24 Mo3 O18 K2 61.5(17) . 2
O4 Mo3 O18 K2 -37.4(16) . 2
O1 Mo3 O18 K2 160.1(14) . 2
O2 Mo3 O18 K2 -124.2(14) 1_455 2
O12 Mo3 O18 K2 -69(5) . 2
Mo4 Mo3 O18 K2 -160.3(13) 1_455 2
K1 Mo3 O18 K2 84.7(14) 1_565 2
K1 Mo3 O18 K2 123.0(13) 2_556 2
O24 Mo3 O18 K1 -23.2(10) . 1_565
O4 Mo3 O18 K1 -122.1(7) . 1_565
O1 Mo3 O18 K1 75.3(8) . 1_565
O2 Mo3 O18 K1 151.1(7) 1_455 1_565
O12 Mo3 O18 K1 -154(5) . 1_565
Mo4 Mo3 O18 K1 115.0(4) 1_455 1_565
K1 Mo3 O18 K1 38.3(16) 2_556 1_565
O11 Mo4 O19 Th2 122(2) . .
O8 Mo4 O19 Th2 -138(2) . .
O2 Mo4 O19 Th2 15(2) . .
O1 Mo4 O19 Th2 -35(5) 1_655 .
O13 Mo4 O19 Th2 -61(2) . .
Mo3 Mo4 O19 Th2 17(3) 1_655 .
Th1 Mo4 O19 Th2 -151.7(13) 2_666 .
Th1 Mo4 O19 Th2 -100(2) . .
K2 Mo4 O19 Th2 135(2) 2 .
O11 Mo4 O19 K2 -13.1(10) . 2
O8 Mo4 O19 K2 87.3(8) . 2
O2 Mo4 O19 K2 -119.4(8) . 2
O1 Mo4 O19 K2 -169(3) 1_655 2
O13 Mo4 O19 K2 164.5(8) . 2
Mo3 Mo4 O19 K2 -117.5(7) 1_655 2
Th1 Mo4 O19 K2 73.6(13) 2_666 2
Th1 Mo4 O19 K2 124.8(6) . 2
O10 Th2 O19 Mo4 -136(2) 2 .
O16 Th2 O19 Mo4 175.6(17) 1_455 .
O23 Th2 O19 Mo4 -59(2) 2_655 .
O7 Th2 O19 Mo4 -14(3) . .
O21 Th2 O19 Mo4 24(2) . .
O6 Th2 O19 Mo4 86(2) . .
O4 Th2 O19 Mo4 136(2) . .
Mo6 Th2 O19 Mo4 -44(2) . .
Mo2 Th2 O19 Mo4 103(2) . .
K2 Th2 O19 Mo4 -134(3) 2 .
Sr1 Th2 O19 Mo4 111(2) . .
O10 Th2 O19 K2 -2.8(7) 2 2
O16 Th2 O19 K2 -50.7(17) 1_455 2
O23 Th2 O19 K2 75.0(7) 2_655 2
O7 Th2 O19 K2 119.9(9) . 2
O21 Th2 O19 K2 157.7(9) . 2
O6 Th2 O19 K2 -140.5(7) . 2
O4 Th2 O19 K2 -90.1(8) . 2
Mo6 Th2 O19 K2 89.2(7) . 2
Mo2 Th2 O19 K2 -122.9(6) . 2
Sr1 Th2 O19 K2 -115.0(7) . 2
O22 Mo5 O20 Mo6 -80.2(11) . .
O16 Mo5 O20 Mo6 175.1(11) . .
O23 Mo5 O20 Mo6 72(2) . .
O14 Mo5 O20 Mo6 18.9(9) . .
O14 Mo5 O20 Mo6 93.0(10) 2_655 .
Sr1 Mo5 O20 Mo6 -147.7(13) 1_655 .
O22 Mo5 O20 Sr1 67.5(10) . 1_655
O16 Mo5 O20 Sr1 -37.2(9) . 1_655
O23 Mo5 O20 Sr1 -140.5(17) . 1_655
O14 Mo5 O20 Sr1 166.6(10) . 1_655
O14 Mo5 O20 Sr1 -119.3(8) 2_655 1_655
Mo6 Mo5 O20 Sr1 147.7(13) . 1_655
O17 Mo6 O20 Mo5 83.8(11) . .
O10 Mo6 O20 Mo5 -47(3) . .
O7 Mo6 O20 Mo5 -175.5(10) . .
O14 Mo6 O20 Mo5 -18.3(9) . .
O23 Mo6 O20 Mo5 -96.6(10) 2_655 .
Th2 Mo6 O20 Mo5 -136.0(8) . .
K2 Mo6 O20 Mo5 86.8(14) . .
K2 Mo6 O20 Mo5 154.2(10) 2_545 .
Sr1 Mo6 O20 Mo5 62.3(8) 2_545 .
O17 Mo6 O20 Sr1 -40.7(18) . 1_655
O10 Mo6 O20 Sr1 -171.5(16) . 1_655
O7 Mo6 O20 Sr1 60.0(16) . 1_655
O14 Mo6 O20 Sr1 -142.8(18) . 1_655
O23 Mo6 O20 Sr1 138.9(17) 2_655 1_655
Mo5 Mo6 O20 Sr1 -125(2) . 1_655
Th2 Mo6 O20 Sr1 99.5(15) . 1_655
K2 Mo6 O20 Sr1 -38(2) . 1_655
K2 Mo6 O20 Sr1 29.7(14) 2_545 1_655
Sr1 Mo6 O20 Sr1 -62.2(15) 2_545 1_655
O5 Mo1 O21 Th2 131(2) . .
O3 Mo1 O21 Th2 -127(2) . .
O13 Mo1 O21 Th2 26(2) . .
O12 Mo1 O21 Th2 -65(3) 1_655 .
O2 Mo1 O21 Th2 -46(2) . .
Mo2 Mo1 O21 Th2 -124(2) 1_655 .
K1 Mo1 O21 Th2 32(3) 2_656 .
K1 Mo1 O21 Th2 115(2) . .
O10 Th2 O21 Mo1 42(3) 2 .
O16 Th2 O21 Mo1 -155(2) 1_455 .
O19 Th2 O21 Mo1 4(2) . .
O23 Th2 O21 Mo1 89(2) 2_655 .
O7 Th2 O21 Mo1 158(3) . .
O6 Th2 O21 Mo1 -116(2) . .
O4 Th2 O21 Mo1 -60(2) . .
Mo6 Th2 O21 Mo1 130(2) . .
Mo2 Th2 O21 Mo1 -88(2) . .
K2 Th2 O21 Mo1 20(2) 2 .
Sr1 Th2 O21 Mo1 -137(2) . .
O16 Mo5 O22 Sr1 134.9(16) . 2_545
O23 Mo5 O22 Sr1 -120.6(15) . 2_545
O20 Mo5 O22 Sr1 47.6(17) . 2_545
O14 Mo5 O22 Sr1 -28.9(17) . 2_545
O14 Mo5 O22 Sr1 -49(9) 2_655 2_545
Mo6 Mo5 O22 Sr1 10.4(15) . 2_545
Sr1 Mo5 O22 Sr1 92.0(15) 1_655 2_545
O16 Mo5 O22 K2 -64.0(15) . 1_655
O23 Mo5 O22 K2 40.5(14) . 1_655
O20 Mo5 O22 K2 -151.4(12) . 1_655
O14 Mo5 O22 K2 132.2(13) . 1_655
O14 Mo5 O22 K2 112(8) 2_655 1_655
Mo6 Mo5 O22 K2 171.5(12) . 1_655
Sr1 Mo5 O22 K2 -106.9(12) 1_655 1_655
O22 Mo5 O23 Mo6 -175.7(9) . 2_655
O16 Mo5 O23 Mo6 -67.4(11) . 2_655
O20 Mo5 O23 Mo6 32(2) . 2_655
O14 Mo5 O23 Mo6 82.8(9) . 2_655
O14 Mo5 O23 Mo6 10.9(8) 2_655 2_655
Mo6 Mo5 O23 Mo6 81.2(9) . 2_655
Sr1 Mo5 O23 Mo6 -84.2(13) 1_655 2_655
O22 Mo5 O23 Th2 -34(2) . 2_655
O16 Mo5 O23 Th2 74.4(19) . 2_655
O20 Mo5 O23 Th2 174.3(15) . 2_655
O14 Mo5 O23 Th2 -135.4(18) . 2_655
O14 Mo5 O23 Th2 152.7(19) 2_655 2_655
Mo6 Mo5 O23 Th2 -137.0(14) . 2_655
Sr1 Mo5 O23 Th2 58(2) 1_655 2_655
O18 Mo3 O24 Th1 -114(3) . .
O4 Mo3 O24 Th1 -15(3) . .
O1 Mo3 O24 Th1 143(2) . .
O2 Mo3 O24 Th1 80(4) 1_455 .
O12 Mo3 O24 Th1 58(2) . .
Mo4 Mo3 O24 Th1 135(2) 1_455 .
K1 Mo3 O24 Th1 -142(3) 1_565 .
K1 Mo3 O24 Th1 98(3) 2_556 .
O18 Mo3 O24 K1 28.2(12) . 1_565
O4 Mo3 O24 K1 127.1(9) . 1_565
O1 Mo3 O24 K1 -75.4(10) . 1_565
O2 Mo3 O24 K1 -138.1(18) 1_455 1_565
O12 Mo3 O24 K1 -159.9(9) . 1_565
Mo4 Mo3 O24 K1 -83.1(11) 1_455 1_565
K1 Mo3 O24 K1 -120.4(9) 2_556 1_565
O13 Th1 O24 Mo3 51(3) . .
O9 Th1 O24 Mo3 -16(2) . .
O15 Th1 O24 Mo3 -90(3) 2_556 .
O1 Th1 O24 Mo3 -167(3) 2_566 .
O8 Th1 O24 Mo3 107(3) . .
O5 Th1 O24 Mo3 -51(4) 2_656 .
O8 Th1 O24 Mo3 148(2) 2_666 .
Mo4 Th1 O24 Mo3 -179(2) 2_666 .
Mo4 Th1 O24 Mo3 77(3) . .
K1 Th1 O24 Mo3 97(3) 2_656 .
K1 Th1 O24 Mo3 143(3) 1_565 .
O13 Th1 O24 K1 -91.3(8) . 1_565
O9 Th1 O24 K1 -158.6(9) . 1_565
O15 Th1 O24 K1 127.3(8) 2_556 1_565
O1 Th1 O24 K1 50.1(7) 2_566 1_565
O8 Th1 O24 K1 -35.8(7) . 1_565
O5 Th1 O24 K1 166.7(14) 2_656 1_565
O8 Th1 O24 K1 5.5(11) 2_666 1_565
Mo4 Th1 O24 K1 38.6(8) 2_666 1_565
Mo4 Th1 O24 K1 -65.4(6) . 1_565
K1 Th1 O24 K1 -45.4(16) 2_656 1_565
Mo2 O6 Sr1 O17 -170.6(9) . 2_545
Th2 O6 Sr1 O17 70.9(8) . 2_545
K1 O6 Sr1 O17 -89.4(8) . 2_545
Mo2 O6 Sr1 O11 -35.7(11) . 1_445
Th2 O6 Sr1 O11 -154.2(7) . 1_445
K1 O6 Sr1 O11 45.5(9) . 1_445
Mo2 O6 Sr1 O3 21.9(8) . 1_455
Th2 O6 Sr1 O3 -96.6(9) . 1_455
K1 O6 Sr1 O3 103.1(9) . 1_455
Mo2 O6 Sr1 O22 -116(4) . 2_545
Th2 O6 Sr1 O22 126(4) . 2_545
K1 O6 Sr1 O22 -35(4) . 2_545
Mo2 O6 Sr1 O20 77.5(10) . 1_455
Th2 O6 Sr1 O20 -41.0(9) . 1_455
K1 O6 Sr1 O20 158.7(7) . 1_455
Mo2 O6 Sr1 O16 111.2(10) . 1_455
Th2 O6 Sr1 O16 -7.3(7) . 1_455
K1 O6 Sr1 O16 -167.6(10) . 1_455
Mo2 O6 Sr1 O18 -102.6(10) . 1_545
Th2 O6 Sr1 O18 138.9(9) . 1_545
K1 O6 Sr1 O18 -21.4(7) . 1_545
Mo2 O6 Sr1 Mo5 107.2(8) . 1_455
Th2 O6 Sr1 Mo5 -11.3(7) . 1_455
K1 O6 Sr1 Mo5 -171.5(6) . 1_455
Th2 O6 Sr1 Mo2 -118.5(12) . .
K1 O6 Sr1 Mo2 81.2(9) . .
Mo2 O6 Sr1 Mo6 -160.7(6) . 2_545
Th2 O6 Sr1 Mo6 80.8(7) . 2_545
K1 O6 Sr1 Mo6 -79.4(7) . 2_545
Mo2 O6 Sr1 K2 -153.1(10) . 2_545
Th2 O6 Sr1 K2 88.4(7) . 2_545
K1 O6 Sr1 K2 -71.9(6) . 2_545
O15 Mo2 Sr1 O17 -102.9(9) . 2_545
O6 Mo2 Sr1 O17 11.2(11) . 2_545
O9 Mo2 Sr1 O17 -4.4(14) . 2_545
O12 Mo2 Sr1 O17 161.9(9) . 2_545
O3 Mo2 Sr1 O17 156.4(10) 1_455 2_545
O4 Mo2 Sr1 O17 88.2(8) . 2_545
Mo1 Mo2 Sr1 O17 171.7(6) 1_455 2_545
K1 Mo2 Sr1 O17 -50.6(6) . 2_545
Th2 Mo2 Sr1 O17 48.7(6) . 2_545
O15 Mo2 Sr1 O11 32.7(9) . 1_445
O6 Mo2 Sr1 O11 146.8(10) . 1_445
O9 Mo2 Sr1 O11 131.2(13) . 1_445
O12 Mo2 Sr1 O11 -62.6(8) . 1_445
O3 Mo2 Sr1 O11 -68.0(9) 1_455 1_445
O4 Mo2 Sr1 O11 -136.3(7) . 1_445
Mo1 Mo2 Sr1 O11 -52.8(5) 1_455 1_445
K1 Mo2 Sr1 O11 85.0(5) . 1_445
Th2 Mo2 Sr1 O11 -175.7(5) . 1_445
O15 Mo2 Sr1 O3 100.7(11) . 1_455
O6 Mo2 Sr1 O3 -145.2(12) . 1_455
O9 Mo2 Sr1 O3 -160.8(15) . 1_455
O12 Mo2 Sr1 O3 5.5(10) . 1_455
O4 Mo2 Sr1 O3 -68.3(10) . 1_455
Mo1 Mo2 Sr1 O3 15.3(8) 1_455 1_455
K1 Mo2 Sr1 O3 153.0(8) . 1_455
Th2 Mo2 Sr1 O3 -107.7(8) . 1_455
O15 Mo2 Sr1 O22 44.4(15) . 2_545
O6 Mo2 Sr1 O22 158.6(16) . 2_545
O9 Mo2 Sr1 O22 142.9(18) . 2_545
O12 Mo2 Sr1 O22 -50.8(15) . 2_545
O3 Mo2 Sr1 O22 -56.3(15) 1_455 2_545
O4 Mo2 Sr1 O22 -124.5(14) . 2_545
Mo1 Mo2 Sr1 O22 -41.0(13) 1_455 2_545
K1 Mo2 Sr1 O22 96.7(13) . 2_545
Th2 Mo2 Sr1 O22 -164.0(13) . 2_545
O15 Mo2 Sr1 O20 136.4(9) . 1_455
O6 Mo2 Sr1 O20 -109.5(10) . 1_455
O9 Mo2 Sr1 O20 -125.1(13) . 1_455
O12 Mo2 Sr1 O20 41.2(8) . 1_455
O3 Mo2 Sr1 O20 35.7(9) 1_455 1_455
O4 Mo2 Sr1 O20 -32.5(7) . 1_455
Mo1 Mo2 Sr1 O20 51.0(5) 1_455 1_455
K1 Mo2 Sr1 O20 -171.3(5) . 1_455
Th2 Mo2 Sr1 O20 -72.0(5) . 1_455
O15 Mo2 Sr1 O16 -173.2(9) . 1_455
O6 Mo2 Sr1 O16 -59.1(10) . 1_455
O9 Mo2 Sr1 O16 -74.7(13) . 1_455
O12 Mo2 Sr1 O16 91.6(8) . 1_455
O3 Mo2 Sr1 O16 86.1(9) 1_455 1_455
O4 Mo2 Sr1 O16 17.8(7) . 1_455
Mo1 Mo2 Sr1 O16 101.4(5) 1_455 1_455
K1 Mo2 Sr1 O16 -120.9(5) . 1_455
Th2 Mo2 Sr1 O16 -21.6(5) . 1_455
O15 Mo2 Sr1 O6 -114.1(11) . .
O9 Mo2 Sr1 O6 -15.6(15) . .
O12 Mo2 Sr1 O6 150.6(11) . .
O3 Mo2 Sr1 O6 145.2(12) 1_455 .
O4 Mo2 Sr1 O6 76.9(10) . .
Mo1 Mo2 Sr1 O6 160.4(9) 1_455 .
K1 Mo2 Sr1 O6 -61.8(9) . .
Th2 Mo2 Sr1 O6 37.5(9) . .
O15 Mo2 Sr1 O18 -45.3(9) . 1_545
O6 Mo2 Sr1 O18 68.8(10) . 1_545
O9 Mo2 Sr1 O18 53.2(13) . 1_545
O12 Mo2 Sr1 O18 -140.6(8) . 1_545
O3 Mo2 Sr1 O18 -146.0(9) 1_455 1_545
O4 Mo2 Sr1 O18 145.7(7) . 1_545
Mo1 Mo2 Sr1 O18 -130.8(5) 1_455 1_545
K1 Mo2 Sr1 O18 7.0(5) . 1_545
Th2 Mo2 Sr1 O18 106.2(5) . 1_545
O15 Mo2 Sr1 Mo5 170.0(7) . 1_455
O6 Mo2 Sr1 Mo5 -75.9(9) . 1_455
O9 Mo2 Sr1 Mo5 -91.5(12) . 1_455
O12 Mo2 Sr1 Mo5 74.7(7) . 1_455
O3 Mo2 Sr1 Mo5 69.3(8) 1_455 1_455
O4 Mo2 Sr1 Mo5 1.0(5) . 1_455
Mo1 Mo2 Sr1 Mo5 84.55(12) 1_455 1_455
K1 Mo2 Sr1 Mo5 -137.70(17) . 1_455
Th2 Mo2 Sr1 Mo5 -38.42(9) . 1_455
O15 Mo2 Sr1 Mo6 -87.6(7) . 2_545
O6 Mo2 Sr1 Mo6 26.6(9) . 2_545
O9 Mo2 Sr1 Mo6 10.9(13) . 2_545
O12 Mo2 Sr1 Mo6 177.2(7) . 2_545
O3 Mo2 Sr1 Mo6 171.7(8) 1_455 2_545
O4 Mo2 Sr1 Mo6 103.5(6) . 2_545
Mo1 Mo2 Sr1 Mo6 -173.0(2) 1_455 2_545
K1 Mo2 Sr1 Mo6 -35.3(3) . 2_545
Th2 Mo2 Sr1 Mo6 64.0(2) . 2_545
O15 Mo2 Sr1 K2 -91.6(7) . 2_545
O6 Mo2 Sr1 K2 22.5(9) . 2_545
O9 Mo2 Sr1 K2 6.9(12) . 2_545
O12 Mo2 Sr1 K2 173.2(7) . 2_545
O3 Mo2 Sr1 K2 167.7(8) 1_455 2_545
O4 Mo2 Sr1 K2 99.4(5) . 2_545
Mo1 Mo2 Sr1 K2 -177.04(15) 1_455 2_545
K1 Mo2 Sr1 K2 -39.3(2) . 2_545
Th2 Mo2 Sr1 K2 59.99(14) . 2_545
Mo2 O15 K1 O12 105.8(8) . 2_556
Th1 O15 K1 O12 -56.4(8) 2_556 2_556
Mo2 O15 K1 O8 -122.8(13) . 1_545
Th1 O15 K1 O8 75.0(16) 2_556 1_545
Mo2 O15 K1 O5 10.7(12) . .
Th1 O15 K1 O5 -151.5(7) 2_556 .
Mo2 O15 K1 O24 -149.1(8) . 1_545
Th1 O15 K1 O24 48.7(9) 2_556 1_545
Mo2 O15 K1 O9 28.1(6) . .
Th1 O15 K1 O9 -134.1(10) 2_556 .
Mo2 O15 K1 O1 155.1(7) . 2_556
Th1 O15 K1 O1 -7.1(10) 2_556 2_556
Mo2 O15 K1 O13 98.3(10) . 2_656
Th1 O15 K1 O13 -63.8(12) 2_556 2_656
Mo2 O15 K1 O18 -101.4(9) . 1_545
Th1 O15 K1 O18 96.4(9) 2_556 1_545
Mo2 O15 K1 O6 -35.2(6) . .
Th1 O15 K1 O6 162.7(11) 2_556 .
Th1 O15 K1 Mo2 -162.2(13) 2_556 .
Mo2 O15 K1 Mo3 -130.6(8) . 1_545
Th1 O15 K1 Mo3 67.2(7) 2_556 1_545
Mo1 O5 K1 O12 -109.2(11) . 2_556
Th1 O5 K1 O12 81.6(7) 2_656 2_556
Mo1 O5 K1 O8 135.6(12) . 1_545
Th1 O5 K1 O8 -33.5(6) 2_656 1_545
Mo1 O5 K1 O15 -22.5(15) . .
Th1 O5 K1 O15 168.4(7) 2_656 .
Mo1 O5 K1 O24 129.8(11) . 1_545
Th1 O5 K1 O24 -39.4(10) 2_656 1_545
Mo1 O5 K1 O9 -37.3(10) . .
Th1 O5 K1 O9 153.5(7) 2_656 .
Mo1 O5 K1 O1 -168.4(10) . 2_556
Th1 O5 K1 O1 22.5(7) 2_656 2_556
Mo1 O5 K1 O13 -149.2(13) . 2_656
Th1 O5 K1 O13 41.6(5) 2_656 2_656
Mo1 O5 K1 O18 62.7(13) . 1_545
Th1 O5 K1 O18 -106.5(7) 2_656 1_545
Mo1 O5 K1 O6 11.9(11) . .
Th1 O5 K1 O6 -157.3(6) 2_656 .
Mo1 O5 K1 Mo2 -16.9(11) . .
Th1 O5 K1 Mo2 174.0(4) 2_656 .
Mo1 O5 K1 Mo3 91.0(12) . 1_545
Th1 O5 K1 Mo3 -78.2(8) 2_656 1_545
Mo2 O9 K1 O12 -117.2(8) . 2_556
Th1 O9 K1 O12 52.3(9) . 2_556
Mo2 O9 K1 O8 126.7(11) . 1_545
Th1 O9 K1 O8 -63.8(15) . 1_545
Mo2 O9 K1 O15 -28.1(7) . .
Th1 O9 K1 O15 141.4(11) . .
Mo2 O9 K1 O5 138.8(8) . .
Th1 O9 K1 O5 -51.7(9) . .
Mo2 O9 K1 O24 -22.8(16) . 1_545
Th1 O9 K1 O24 146.7(11) . 1_545
Mo2 O9 K1 O1 -119.1(8) . 2_556
Th1 O9 K1 O1 50.3(12) . 2_556
Mo2 O9 K1 O13 -166.6(7) . 2_656
Th1 O9 K1 O13 2.9(10) . 2_656
Mo2 O9 K1 O18 18.6(8) . 1_545
Th1 O9 K1 O18 -171.9(8) . 1_545
Mo2 O9 K1 O6 37.5(6) . .
Th1 O9 K1 O6 -153.0(12) . .
Th1 O9 K1 Mo2 169.5(14) . .
Mo2 O9 K1 Mo3 -3.8(9) . 1_545
Th1 O9 K1 Mo3 165.7(6) . 1_545
Mo2 O6 K1 O12 -10.0(9) . 2_556
Th2 O6 K1 O12 96.1(11) . 2_556
Sr1 O6 K1 O12 -108.9(8) . 2_556
Mo2 O6 K1 O8 -178.3(7) . 1_545
Th2 O6 K1 O8 -72.2(11) . 1_545
Sr1 O6 K1 O8 82.8(9) . 1_545
Mo2 O6 K1 O15 36.1(7) . .
Th2 O6 K1 O15 142.2(12) . .
Sr1 O6 K1 O15 -62.8(8) . .
Mo2 O6 K1 O5 -112.0(7) . .
Th2 O6 K1 O5 -5.9(10) . .
Sr1 O6 K1 O5 149.1(8) . .
Mo2 O6 K1 O24 112.4(8) . 1_545
Th2 O6 K1 O24 -141.5(10) . 1_545
Sr1 O6 K1 O24 13.5(10) . 1_545
Mo2 O6 K1 O9 -38.6(6) . .
Th2 O6 K1 O9 67.5(10) . .
Sr1 O6 K1 O9 -137.5(10) . .
Mo2 O6 K1 O1 69(2) . 2_556
Th2 O6 K1 O1 174.9(15) . 2_556
Sr1 O6 K1 O1 -30(2) . 2_556
Mo2 O6 K1 O13 -82.9(11) . 2_656
Th2 O6 K1 O13 23.3(16) . 2_656
Sr1 O6 K1 O13 178.3(7) . 2_656
Mo2 O6 K1 O18 119.5(9) . 1_545
Th2 O6 K1 O18 -134.4(12) . 1_545
Sr1 O6 K1 O18 20.6(7) . 1_545
Th2 O6 K1 Mo2 106.1(12) . .
Sr1 O6 K1 Mo2 -98.9(9) . .
Mo2 O6 K1 Mo3 107.7(6) . 1_545
Th2 O6 K1 Mo3 -146.1(9) . 1_545
Sr1 O6 K1 Mo3 8.8(6) . 1_545
O15 Mo2 K1 O12 -71.8(9) . 2_556
O6 Mo2 K1 O12 171.4(8) . 2_556
O9 Mo2 K1 O12 59.1(8) . 2_556
O12 Mo2 K1 O12 -4.6(12) . 2_556
O3 Mo2 K1 O12 -118.2(9) 1_455 2_556
O4 Mo2 K1 O12 112.1(8) . 2_556
Mo1 Mo2 K1 O12 -66.1(5) 1_455 2_556
Th2 Mo2 K1 O12 140.2(4) . 2_556
Sr1 Mo2 K1 O12 -145.6(5) . 2_556
O15 Mo2 K1 O8 119.9(13) . 1_545
O6 Mo2 K1 O8 3.1(12) . 1_545
O9 Mo2 K1 O8 -109.2(13) . 1_545
O12 Mo2 K1 O8 -172.9(12) . 1_545
O3 Mo2 K1 O8 73.5(14) 1_455 1_545
O4 Mo2 K1 O8 -56.2(13) . 1_545
Mo1 Mo2 K1 O8 125.6(10) 1_455 1_545
Th2 Mo2 K1 O8 -28.1(11) . 1_545
Sr1 Mo2 K1 O8 46.1(11) . 1_545
O6 Mo2 K1 O15 -116.8(10) . .
O9 Mo2 K1 O15 131.0(11) . .
O12 Mo2 K1 O15 67.3(11) . .
O3 Mo2 K1 O15 -46.4(12) 1_455 .
O4 Mo2 K1 O15 -176.1(11) . .
Mo1 Mo2 K1 O15 5.7(8) 1_455 .
Th2 Mo2 K1 O15 -148.0(8) . .
Sr1 Mo2 K1 O15 -73.8(8) . .
O15 Mo2 K1 O5 -172.0(9) . .
O6 Mo2 K1 O5 71.2(8) . .
O9 Mo2 K1 O5 -41.0(8) . .
O12 Mo2 K1 O5 -104.8(9) . .
O3 Mo2 K1 O5 141.6(9) 1_455 .
O4 Mo2 K1 O5 11.9(9) . .
Mo1 Mo2 K1 O5 -166.3(4) 1_455 .
Th2 Mo2 K1 O5 40.0(4) . .
Sr1 Mo2 K1 O5 114.2(4) . .
O15 Mo2 K1 O24 35.7(10) . 1_545
O6 Mo2 K1 O24 -81.1(9) . 1_545
O9 Mo2 K1 O24 166.7(10) . 1_545
O12 Mo2 K1 O24 102.9(9) . 1_545
O3 Mo2 K1 O24 -10.7(10) 1_455 1_545
O4 Mo2 K1 O24 -140.4(9) . 1_545
Mo1 Mo2 K1 O24 41.4(7) 1_455 1_545
Th2 Mo2 K1 O24 -112.3(6) . 1_545
Sr1 Mo2 K1 O24 -38.1(6) . 1_545
O15 Mo2 K1 O9 -131.0(11) . .
O6 Mo2 K1 O9 112.2(10) . .
O12 Mo2 K1 O9 -63.7(10) . .
O3 Mo2 K1 O9 -177.3(11) 1_455 .
O4 Mo2 K1 O9 53.0(10) . .
Mo1 Mo2 K1 O9 -125.3(7) 1_455 .
Th2 Mo2 K1 O9 81.0(7) . .
Sr1 Mo2 K1 O9 155.3(7) . .
O15 Mo2 K1 O1 -37.0(10) . 2_556
O6 Mo2 K1 O1 -153.8(10) . 2_556
O9 Mo2 K1 O1 94.0(10) . 2_556
O12 Mo2 K1 O1 30.3(11) . 2_556
O3 Mo2 K1 O1 -83.4(11) 1_455 2_556
O4 Mo2 K1 O1 147.0(9) . 2_556
Mo1 Mo2 K1 O1 -31.3(8) 1_455 2_556
Th2 Mo2 K1 O1 175.0(7) . 2_556
Sr1 Mo2 K1 O1 -110.8(7) . 2_556
O15 Mo2 K1 O13 -113.1(10) . 2_656
O6 Mo2 K1 O13 130.1(9) . 2_656
O9 Mo2 K1 O13 17.9(9) . 2_656
O12 Mo2 K1 O13 -45.8(10) . 2_656
O3 Mo2 K1 O13 -159.5(9) 1_455 2_656
O4 Mo2 K1 O13 70.9(9) . 2_656
Mo1 Mo2 K1 O13 -107.4(6) 1_455 2_656
Th2 Mo2 K1 O13 98.9(6) . 2_656
Sr1 Mo2 K1 O13 173.1(6) . 2_656
O15 Mo2 K1 O18 67.6(9) . 1_545
O6 Mo2 K1 O18 -49.1(8) . 1_545
O9 Mo2 K1 O18 -161.4(8) . 1_545
O12 Mo2 K1 O18 134.9(9) . 1_545
O3 Mo2 K1 O18 21.3(9) 1_455 1_545
O4 Mo2 K1 O18 -108.4(8) . 1_545
Mo1 Mo2 K1 O18 73.4(5) 1_455 1_545
Th2 Mo2 K1 O18 -80.4(4) . 1_545
Sr1 Mo2 K1 O18 -6.1(4) . 1_545
O15 Mo2 K1 O6 116.8(10) . .
O9 Mo2 K1 O6 -112.2(10) . .
O12 Mo2 K1 O6 -176.0(10) . .
O3 Mo2 K1 O6 70.4(10) 1_455 .
O4 Mo2 K1 O6 -59.3(10) . .
Mo1 Mo2 K1 O6 122.5(7) 1_455 .
Th2 Mo2 K1 O6 -31.2(7) . .
Sr1 Mo2 K1 O6 43.0(7) . .
O15 Mo2 K1 Mo3 45.9(8) . 1_545
O6 Mo2 K1 Mo3 -70.9(7) . 1_545
O9 Mo2 K1 Mo3 176.9(7) . 1_545
O12 Mo2 K1 Mo3 113.2(7) . 1_545
O3 Mo2 K1 Mo3 -0.5(8) 1_455 1_545
O4 Mo2 K1 Mo3 -130.1(7) . 1_545
Mo1 Mo2 K1 Mo3 51.6(3) 1_455 1_545
Th2 Mo2 K1 Mo3 -102.11(13) . 1_545
Sr1 Mo2 K1 Mo3 -27.86(17) . 1_545
Mo6 O17 K2 O7 -132.4(10) . 2_545
Sr1 O17 K2 O7 82.4(7) 2_545 2_545
Mo6 O17 K2 O11 31(7) . 2
Sr1 O17 K2 O11 -115(6) 2_545 2
Mo6 O17 K2 O10 14.7(7) . .
Sr1 O17 K2 O10 -130.5(9) 2_545 .
Mo6 O17 K2 O19 45.5(11) . 2
Sr1 O17 K2 O19 -99.7(8) 2_545 2
Mo6 O17 K2 O22 -42.5(11) . 1_455
Sr1 O17 K2 O22 172.3(7) 2_545 1_455
Mo6 O17 K2 O18 101.4(10) . 2
Sr1 O17 K2 O18 -43.8(7) 2_545 2
Sr1 O17 K2 Mo6 -145.2(13) 2_545 .
Mo6 O17 K2 Mo4 51.9(14) . 2
Sr1 O17 K2 Mo4 -93.2(9) 2_545 2
Mo6 O17 K2 Mo6 -110.0(8) . 2_545
Sr1 O17 K2 Mo6 104.9(6) 2_545 2_545
Mo6 O17 K2 Sr1 145.2(13) . 2_545
Mo6 O17 K2 Sr1 -80.3(12) . 2_445
Sr1 O17 K2 Sr1 134.5(7) 2_545 2_445
Mo6 O10 K2 O7 25.7(11) . 2_545
Th2 O10 K2 O7 -167.9(7) 2 2_545
Mo6 O10 K2 O17 -13.7(7) . .
Th2 O10 K2 O17 152.7(10) 2 .
Mo6 O10 K2 O11 168.4(8) . 2
Th2 O10 K2 O11 -25.2(10) 2 2
Mo6 O10 K2 O19 -163.8(10) . 2
Th2 O10 K2 O19 2.6(7) 2 2
Mo6 O10 K2 O22 116.8(9) . 1_455
Th2 O10 K2 O22 -76.8(8) 2 1_455
Mo6 O10 K2 O18 -87.1(8) . 2
Th2 O10 K2 O18 79.2(8) 2 2
Th2 O10 K2 Mo6 166.4(13) 2 .
Mo6 O10 K2 Mo4 -173.6(7) . 2
Th2 O10 K2 Mo4 -7.2(7) 2 2
Mo6 O10 K2 Mo6 49.7(8) . 2_545
Th2 O10 K2 Mo6 -143.9(5) 2 2_545
Mo6 O10 K2 Sr1 -41.6(7) . 2_545
Th2 O10 K2 Sr1 124.8(7) 2 2_545
Mo6 O10 K2 Sr1 125.8(6) . 2_445
Th2 O10 K2 Sr1 -67.8(8) 2 2_445
O17 Mo6 K2 O7 46.2(10) . 2_545
O10 Mo6 K2 O7 -158.7(10) . 2_545
O7 Mo6 K2 O7 -55.9(9) . 2_545
O20 Mo6 K2 O7 42.3(13) . 2_545
O14 Mo6 K2 O7 134.5(8) . 2_545
O23 Mo6 K2 O7 -132.9(8) 2_655 2_545
Mo5 Mo6 K2 O7 94.1(5) . 2_545
Th2 Mo6 K2 O7 -92.3(5) . 2_545
K2 Mo6 K2 O7 -23.0(4) 2_545 2_545
Sr1 Mo6 K2 O7 69.4(5) 2_545 2_545
O10 Mo6 K2 O17 155.1(12) . .
O7 Mo6 K2 O17 -102.1(11) . .
O20 Mo6 K2 O17 -3.9(15) . .
O14 Mo6 K2 O17 88.3(11) . .
O23 Mo6 K2 O17 -179.1(12) 2_655 .
Mo5 Mo6 K2 O17 47.9(9) . .
Th2 Mo6 K2 O17 -138.5(9) . .
K2 Mo6 K2 O17 -69.2(9) 2_545 .
Sr1 Mo6 K2 O17 23.2(9) 2_545 .
O17 Mo6 K2 O11 -173.8(14) . 2
O10 Mo6 K2 O11 -18.7(12) . 2
O7 Mo6 K2 O11 84.1(11) . 2
O20 Mo6 K2 O11 -177.7(15) . 2
O14 Mo6 K2 O11 -85.5(12) . 2
O23 Mo6 K2 O11 7.1(13) 2_655 2
Mo5 Mo6 K2 O11 -125.9(10) . 2
Th2 Mo6 K2 O11 47.7(10) . 2
K2 Mo6 K2 O11 117.1(10) 2_545 2
Sr1 Mo6 K2 O11 -150.5(10) 2_545 2
O17 Mo6 K2 O10 -155.1(12) . .
O7 Mo6 K2 O10 102.8(10) . .
O20 Mo6 K2 O10 -159.0(14) . .
O14 Mo6 K2 O10 -66.8(10) . .
O23 Mo6 K2 O10 25.8(11) 2_655 .
Mo5 Mo6 K2 O10 -107.2(8) . .
Th2 Mo6 K2 O10 66.4(8) . .
K2 Mo6 K2 O10 135.7(8) 2_545 .
Sr1 Mo6 K2 O10 -131.9(8) 2_545 .
O17 Mo6 K2 O19 -140.2(11) . 2
O10 Mo6 K2 O19 14.9(9) . 2
O7 Mo6 K2 O19 117.7(7) . 2
O20 Mo6 K2 O19 -144.1(13) . 2
O14 Mo6 K2 O19 -51.8(8) . 2
O23 Mo6 K2 O19 40.7(9) 2_655 2
Mo5 Mo6 K2 O19 -92.3(5) . 2
Th2 Mo6 K2 O19 81.3(5) . 2
K2 Mo6 K2 O19 150.7(5) 2_545 2
Sr1 Mo6 K2 O19 -116.9(5) 2_545 2
O17 Mo6 K2 O22 142.7(11) . 1_455
O10 Mo6 K2 O22 -62.2(9) . 1_455
O7 Mo6 K2 O22 40.5(8) . 1_455
O20 Mo6 K2 O22 138.7(13) . 1_455
O14 Mo6 K2 O22 -129.0(8) . 1_455
O23 Mo6 K2 O22 -36.5(9) 2_655 1_455
Mo5 Mo6 K2 O22 -169.4(5) . 1_455
Th2 Mo6 K2 O22 4.2(5) . 1_455
K2 Mo6 K2 O22 73.5(5) 2_545 1_455
Sr1 Mo6 K2 O22 165.9(5) 2_545 1_455
O17 Mo6 K2 O18 -69.9(10) . 2
O10 Mo6 K2 O18 85.2(9) . 2
O7 Mo6 K2 O18 -172.1(8) . 2
O20 Mo6 K2 O18 -73.9(13) . 2
O14 Mo6 K2 O18 18.4(8) . 2
O23 Mo6 K2 O18 110.9(9) 2_655 2
Mo5 Mo6 K2 O18 -22.0(5) . 2
Th2 Mo6 K2 O18 151.6(5) . 2
K2 Mo6 K2 O18 -139.1(5) 2_545 2
Sr1 Mo6 K2 O18 -46.7(5) 2_545 2
O17 Mo6 K2 Mo4 -147.4(10) . 2
O10 Mo6 K2 Mo4 7.7(8) . 2
O7 Mo6 K2 Mo4 110.5(6) . 2
O20 Mo6 K2 Mo4 -151.3(12) . 2
O14 Mo6 K2 Mo4 -59.1(7) . 2
O23 Mo6 K2 Mo4 33.5(8) 2_655 2
Mo5 Mo6 K2 Mo4 -99.5(3) . 2
Th2 Mo6 K2 Mo4 74.1(3) . 2
K2 Mo6 K2 Mo4 143.5(4) 2_545 2
Sr1 Mo6 K2 Mo4 -124.1(3) 2_545 2
O17 Mo6 K2 Mo6 69.2(9) . 2_545
O10 Mo6 K2 Mo6 -135.7(8) . 2_545
O7 Mo6 K2 Mo6 -32.9(6) . 2_545
O20 Mo6 K2 Mo6 65.2(12) . 2_545
O14 Mo6 K2 Mo6 157.5(6) . 2_545
O23 Mo6 K2 Mo6 -110.0(7) 2_655 2_545
Mo5 Mo6 K2 Mo6 117.07(16) . 2_545
Th2 Mo6 K2 Mo6 -69.33(16) . 2_545
K2 Mo6 K2 Mo6 0.0 2_545 2_545
Sr1 Mo6 K2 Mo6 92.41(17) 2_545 2_545
O17 Mo6 K2 Sr1 -23.2(9) . 2_545
O10 Mo6 K2 Sr1 131.9(8) . 2_545
O7 Mo6 K2 Sr1 -125.4(6) . 2_545
O20 Mo6 K2 Sr1 -27.2(12) . 2_545
O14 Mo6 K2 Sr1 65.1(7) . 2_545
O23 Mo6 K2 Sr1 157.6(7) 2_655 2_545
Mo5 Mo6 K2 Sr1 24.7(2) . 2_545
Th2 Mo6 K2 Sr1 -161.75(10) . 2_545
K2 Mo6 K2 Sr1 -92.42(17) 2_545 2_545
O17 Mo6 K2 Sr1 130.1(10) . 2_445
O10 Mo6 K2 Sr1 -74.8(8) . 2_445
O7 Mo6 K2 Sr1 28.0(7) . 2_445
O20 Mo6 K2 Sr1 126.2(12) . 2_445
O14 Mo6 K2 Sr1 -141.6(7) . 2_445
O23 Mo6 K2 Sr1 -49.0(8) 2_655 2_445
Mo5 Mo6 K2 Sr1 178.0(2) . 2_445
Th2 Mo6 K2 Sr1 -8.4(3) . 2_445
K2 Mo6 K2 Sr1 60.9(3) 2_545 2_445
Sr1 Mo6 K2 Sr1 153.3(4) 2_545 2_445
